MICROMECHANICSBASED PREDICTION OF THERMOELASTIC PROPERTIES OF HIGH ENERGY MATERIALS


 Edgar Gilmore
 1 years ago
 Views:
Transcription
1 MICROMECHANICSBASED PREDICTION OF THERMOELASTIC PROPERTIES OF HIGH ENERGY MATERIALS by Biswajit Banerjee A dissertation submitted to the faculty of The University of Utah in partial fulfillment of the requirements for the degree of Doctor of Philosophy Department of Mechanical Engineering The University of Utah December 2002
2 Copyright c Biswajit Banerjee 2002 All Rights Reserved
3 THE UNIVERSITY OF UTAH GRADUATE SCHOOL SUPERVISORY COMMITTEE APPROVAL of a dissertation submitted by Biswajit Banerjee This dissertation has been read by each member of the following supervisory committee and by majority vote has been found to be satisfactory. Chair: Daniel O. Adams Lawrence K. DeVries Patrick A. McMurtry Graeme W. Milton John A. Nairn
4 THE UNIVERSITY OF UTAH GRADUATE SCHOOL FINAL READING APPROVAL To the Graduate Council of the University of Utah: I have read the dissertation of Biswajit Banerjee in its final form and have found that (1) its format, citations, and bibliographic style are consistent and acceptable; (2) its illustrative materials including figures, tables, and charts are in place; and (3) the final manuscript is satisfactory to the Supervisory Committee and is ready for submission to The Graduate School. Date Daniel O. Adams Chair, Supervisory Committee Approved for the Major Department Joseph C. Kelwicki Chair/Dean Approved for the Graduate Council David S. Chapman Dean of The Graduate School
5 ABSTRACT High energy materials are used as propellants in solid rockets. Multiscale simulations of these materials require techniques that can bridge submicron scales and engineering scales. Micromechanics provides such techniques. The objective of this research is to investigate micromechanics approaches that can be used estimate the ective thermoelastic properties of high energy materials given the properties of the components. In this research, rigorous bounds and analytical estimates for ective elastic properties are reviewed and applied to mock polymer bonded explosives and the explosive PBX A method of estimating threedimensional elastic properties from twodimensional finite element simulations is presented. Since detailed numerical simulations of PBXs are computationally expensive, two computationally inexpensive techniques are explored: the generalized method of cells and a renormalizationbased approach called the recursive cell method. Results show that rigorous bounds and analytical approximations provide inaccurate estimates of the elastic properties but reasonable estimates of the thermal expansion of PBX Finite element simulations of glassestane composites overestimate the elastic moduli unless particlebinder debonding is included. Results for models of PBX 9501 show that the particle distribution, mesh discretization, and stressbridging affect the estimated properties considerably. The generalized method of cells is shown to underestimate the elastic moduli because of inadequate consideration of stressbridging and shearnormal coupling. The renormalizationbased recursive cell method overestimates the ective properties unless large blocks of subcells are renormalized. Comparisons with exact relations provide useful checks of the accuracy of numerical methods. Detailed numerical simulations appear to be required for the accurate prediction of elastic properties of polymer bonded explosives.
6 To Champa
7 CONTENTS ABSTRACT iv LIST OF TABLES ix LIST OF FIGURES xi ACKNOWLEDGEMENTS xiv CHAPTERS 1. INTRODUCTION Outline of the dissertation BACKGROUND Polymerbonded explosives PBX Elastic properties of PBX Particles  HMX HMX crystal structure Elastic moduli of HMX Thermal expansion of HMX Particle size distribution in PBX Binder  Estane 5703 and BDNPA/F Elastic moduli of PBX 9501 binder Thermal expansion of PBX 9501 binder Mock polymerbonded explosives Micromechanics of composites Rigorous bounds HashinShtrikman bounds Thirdorder bounds Comparison of bounds Analytical methods Composite spheres assemblage (CSA) Selfconsistent schemes (SCS) Differential ective medium approach (DEM) Comparison of analytical approaches Numerical approximations The representative volume element Finite element approximations
8 Homogenization theory Stochastic finite elements Discrete models Integral equation methods Fourier transform method Generalized method of cells MICROMECHANICS SIMULATIONS OF GLASSESTANE MOCK POLYMER BONDED EXPLOSIVES Abstract Introduction GlassEstane mock PBXs  experimental data Estimation of elastic moduli Twodimensional unit cells Effect of unit cell size Threedimensional unit cells Comparison of estimates and experimental data Effect of particle debonding Summary and conclusions EFFECTIVE ELASTIC MODULI OF POLYMER BONDED EXPLOSIVES FROM FINITE ELEMENT SIMULATIONS Abstract Introduction Finite element approach Validation of approach Modeling polymer bonded explosives Manually generated microstructures Randomly generated microstructures Circular particles  PBX 9501 dry blend Circular particles  pressed PBX Square particles  pressed PBX Effective moduli of PBX Summary and conclusions APPLICATION OF THE GENERALIZED METHOD OF CELLS TO POLYMER BONDED EXPLOSIVES Abstract Introduction The generalized method of cells Validation  square arrays of disks Modeling polymer bonded explosives Simplified models of PBX materials Models of PBX StressBridging Corner bridging : Xshaped microstructure vii
9 5.6.2 Edge bridging Summary and conclusions ON PREDICTING THE EFFECTIVE ELASTIC PROPERTIES OF POLYMER METHOD BONDED EXPLOSIVES USING THE RECURSIVE CELL Abstract Introduction Background The recursive cell method Models of particulate composites Models of PBX Percolation Summary and conclusions ON EXACT RELATIONS FOR THE CALCULATION OF EFFECTIVE ELASTIC PROPERTIES OF COMPOSITES Abstract Introduction Phase interchange identity Range of applicability Convergence of FEM calculations Materials rigid in shear Relation RS Relation RS The CLM theorem Composites with equal bulk modulus Hill s equation Summary and conclusions CONCLUSIONS Future work APPENDICES A. TWO AND THREEDIMENSIONAL MODULI 137 B. ELEMENT STIFFNESS MATRICES 139 C. BOUNDARY CONDITIONS 144 D. EFFECTIVE PROPERTIES 149 REFERENCES 151 viii
10 LIST OF TABLES 2.1 Compositions of common PBX materials Weight and volume fractions of the components of PBX Different phases of HMX and transition temperatures The stiffness matrix of HMX Thermal expansion properties of HMX HMX particle size distributions in the PBX 9501 dry blend Elastic moduli and CTE of PBX 9501 and its components at room temperature and low strain rate Bounds on properties of PBX Analytical estimates of properties of PBX Young s modulus of extruded Estane Young s modulus of composites containing glass and estane Effective moduli of the six model PBX 9501 microstructures from FEM calculations sixnoded triangular elements Effective elastic moduli of the four models of the dry blend of PBX Material properties of the dirty binder for the four pressed piece based PBX 9501 microstructures Effective elastic moduli of the four models of pressed PBX Material properties of the dirty binder for the three PBX microstructures with square particles Effective stiffnesses of the model microstructures with square particles Material properties used to calculate the ective moduli of PBX 9501 for different temperatures and strain rates Effective Young s modulus from finite element simulations of a 100 particle model of the dry blend of PBX Component properties used by Greengard and Helsing Experimentally determined elastic moduli and stiffness of PBX 9501 and its constituents Effective stiffnesses of the six model microstructures from GMC and FEM calculations
11 5.4 Effective stiffness of the model PBX 9501 microstructures from GMC and FEM calculations The elastic properties of the components of the Xshaped microstructure Effective properties of edge bridging models Typical polymer bonded explosives Bounds and analytical estimates of the ective elastic properties of PBX Twodimensional ective compliance matrix for a square array of disks Effective compliance matrix for a checkerboard composite with components rigid in shear Original and translated twodimensional constituent moduli for checking the CLM condition Comparison of ective moduli for the original and the translated composites Component properties, exact ective properties and numerically computed ective properties for twocomponent symmetric composite with equal component bulk moduli Phase properties used for testing Hill s equation and the exact ective moduli of the composite Numerically computed ective properties for a square array of disks with equal component shear moduli B.1 Stiffness matrix for the displacement based fournoded element B.2 Stiffness matrix for the displacement based ninenoded element B.3 Stiffness matrix for nine noded mixed displacement/pressure element x
12 LIST OF FIGURES 2.1 Young s modulus of PBX 9501 (a) as a function of strain rate (b) as a function of temperature Monoclinic structure of a HMX crystal HMX particle size distributions in PBX 9501 at various stages of processing Young s modulus of PBX 9501 binder (a) as a function of strain rate (b) as a function of temperature Sample particle distributions and unit cells of various sizes containing 21%, 44% and 59% by volume of monodisperse circular particles Displacement boundary conditions used to calculate the stressstrain behavior of a unit cell Variation of ective elastic properties with the size of the unit cell for a strain rate of 0.001/s and at a temperature of 23 C Threedimensional unit cells containing 21% and 44% by volume of monodisperse circular particles and slices from the unit cells used for threedimensional simulations Young s modulus of glassestane composites from twodimensional and threedimensional unit cell based finite element calculations. The estimates are for a strain rate of 0.001/s Comparison of experimental Young s modulus, bounds and FEM calculations for glassestane composites containing 21% by volume of monodisperse glass beads Comparison of experimental Young s modulus, bounds and FEM calculations for glassestane composites containing 44% by volume of monodisperse glass beads Comparison of experimental Young s modulus, bounds and FEM calculations for glassestane composites containing 59% by volume of monodisperse glass beads Debonded particles under (a) compression and (b) tension for a glassestane composite containing 44% by volume of monodisperse glass beads with three debonded particles. Displacements shown are three times the actual. The applied strain is 1% Effect of particle debonding on predicted values of Young s modulus of 44% glass/56% estane composite (a) under compression (b) under tension. 46
13 4.1 RVEs containing 10% to 92% by volume of circular particles Comparison of finite element and differential ective medium predictions Two and threedimensional RVEs containing 70%, 75% and 80% particles by volume Two and threedimensional estimates of ective Young s modulus and Poisson s ratio Manually generated microstructures containing 90% circular particles by volume Microstructure containing 92% particles modeled with sixnoded triangles and fournoded squares Microstructure of PBX Models based on the dry blend of PBX 9501 containing circular particles Models based on the particle size distribution of pressed PBX 9501 containing circular particles Models with square particles based on the size distribution of pressed PBX RVE, subcells and notation used in GMC Comparison of ective moduli of square arrays of disks from Greengard and Helsing and GMC calculations Manually generated microstructures containing approximately 90% circular particles by volume Schematics of the application of the binary subcell approach and the ective subcell approach in GMC calculations Microstructures containing circular particles based on the particle size distribution of the dry blend (DB) of PBX 9501 and of pressed (PP) PBX RVE used for corner stressbridging model Variation of ective stiffness with modulus contrast for Xshaped microstructure Progressive stressbridging models A through E Stressbridging paths for Model C The recursive cell method.(a) Schematic of the recursive cell method. (b) Recursion procedure applied to a RVE discretized into blocks of four subcells Schematic of normal displacement boundary conditions in used RCM Nine RVEs containing 10% to 92% by volume of circular particles xii
14 6.4 Comparison of finite element (FEM) and RCM predictions for a range of modulus contrasts and volume fractions Microstructure of PBX Model microstructures representing PBX (a) Four microstructures based on the dry blend of PBX (b) Four microstructures based on the size distribution of pressed PBX Effective elastic properties of models of PBX 9501 from RCM calculations High volume fraction model microstructures. (a) Manually generated microstructure with 92% by volume of particles. (b) Automatically generated microstructure with 86% by volume of particles RCM estimates of Young s modulus with increasing subcells per block and the CPU time taken Variation of strain energy density (a) of Models A and B with increasing subcells/block (b) of model B with the number recursions and increasing subcells/block Percolation behavior in high modulus contrast composites from RCM calculations. (a) Effective twodimensional bulk modulus vs. volume fraction ( ). (b) Effective twodimensional bulk modulus vs Percolation behavior in high modulus contrast composites from FEM calculations. (a) Effective twodimensional bulk modulus vs. volume fraction ( ). (b) Effective twodimensional bulk modulus vs Representative volume element for a checkerboard composite Validation of FEM, RCM and GMC using the phase interchange identity for a checkerboard composite Variation of ective shear moduli with modulus contrast for a checkerboard composite Convergence of ective moduli predicted by FEM analyses with increase in mesh refinement for a checkerboard composite with shear modulus contrast of 25, RVE for a square array of disks B.1 Elements using in recursive cell method calculations. (a) Fournoded element (b) Ninenoded element C.1 Schematic of the ect of a uniform displacement applied in the direction.145 C.2 Displacement boundary conditions corresponding to a pure shear. (a) Prescribed displacements are applied at all the boundary nodes. (b) Prescribed displacements are applied only at corner nodes xiii
15 ACKNOWLEDGEMENTS I would like to thank the University of Utah Center for the Simulation of Accidental Fires and Explosions (CSAFE) and Pat McMurtry for supporting this research. Many thanks to my advisor Dan Adams for being supportive of me and my work, for giving me direction and the option of exploring many different avenues, and for speedy turnaround on many iterations of each dissertation chapter during busy times. I would also like to express my gratitude to Graeme Milton for exposing me to numerous theoretical aspects of composites and a voluminous literature on the subject. Thanks to my committee for useful advice and constructive criticism at the proposal defense. Finally, I would like to thank my wife Champa for being supportive of me through this endeavor.
16 CHAPTER 1 INTRODUCTION For many years, scientists have felt the need to predict the behavior of materials from atomistic scales to engineering scales. The recent advent of massively parallel computers and improved simulation techniques have made that goal realistic. Multiscale simulations are usually performed in one of two ways. In the first approach, material behavior is simulated by detailed models at a lower scale and then coarse grained so that this information can be used at a larger scale. The computational approaches can be independent of each other at each scale in this approach. The second approach attempts to link the scales by allowing some interaction between models at different scales. Micromechanics provides a means of coarsegraining information from submicron simulations to engineering scales and can be used in either approach. Highenergy (HE) materials are commonly used as propellants for solid rocket motors. Interest in the mechanical properties of HE materials has developed with improvements in computational capabilities that make possible simulations of containers filled with these materials. Though mechanical properties of HE materials can be determined experimentally, the hazards associated with experiments on these materials, as well as the attending costs, make this option unattractive. Improved numerical and computational techniques make the determination of mechanical properties of HE materials possible by bridging the gaps between atomistic calculations of molecular potentials, molecular dynamics simulations and micromechanics methods for composite materials. In this research, some micromechanicsbased methods for the determination of the mechanical properties of composites are explored and applied to a group of HE materials called polymerbonded explosives (PBXs). PBXs provide unique challenges for micromechanical modeling. These materials
17 2 are viscoelastic particulate composites, contain high volume fractions of particles, and the modulus contrast between the particles and the binder is extremely high. For example, PBX 9501 contains about 92% by volume of particles and the modulus contrast between particles and the binder, at room temperature and low strain rates, is around 20,000. Micromechanics predictions based on analytical approximations are inaccurate because of the high modulus contrast and volume fraction of PBXs. On the other hand, micromechanics predictions from numerical simulations require extremely large grids to accurately capture the microstructure of PBXs. To reduce the complexity of the problem, some simplifying assumptions are made about PBXs in this research. It is assumed that PBXs are twocomponent particulate composites with the particles surrounded by a binder. The components of PBXs are assumed to be isotropic and linear elastic, and only the prediction of elastic moduli and coicients of thermal expansion (CTEs) of PBXs is addressed. Simplified numerical techniques such as the generalized method of cells (GMC) and the recursive cell method (RCM) are explored as alternatives to direct simulations using the finite element method (FEM). The finite element method (FEM) has been used to provide benchmark calculations of ective properties of PBXs. 1.1 Outline of the dissertation A review of the properties of polymer bonded explosives and PBX 9501 is provided in Chapter 2. Rigorous bounds on the ective properties of composites are discussed next and applied to predict the properties of PBX Some analytical approaches are also reviewed and applied to PBX A discussion of various numerical micromechanics methods of predicting the ective properties of composites is provided. Chapter 3 deals with the estimation of ective elastic properties of glassestane mock propellants. The mock material has been chosen because the low volume fraction of glass beads and the monodisperse nature of the beads eliminate two of the variables of concern: high particle volume fractions and different particle sizes. Bounds and numerical estimates using the finite element method for the ective elastic moduli of these composites are obtained and compared to experimental data. The ect of
18 3 the size of the unit cell used in finite element simulations is investigated. Effective properties predicted by two and threedimensional finite element models are compared. In addition, the ect of particlebinder debonding on the ective properties of these composites is explored. In Chapter 4, twodimensional finite element analyses are used to predict the ective properties of high volume fraction polymer bonded explosives such as PBX The approach is validated by way of comparisons with differential ective medium estimates of Young s modulus and predictions from threedimensional finite element models. Various microstructures based on the particle size distribution of PBX 9501 are modeled using twodimensional finite element analysis and the predicted properties are compared with experimental data. A computationally inexpensive alternative to direct finite element simulation for some composites is the generalized method of cells (GMC). Chapter 5 discusses the formulation of GMC and its applicability to polymer bonded explosives. Estimates of ective properties of polymer bonded explosives from GMC are compared to finite element based estimates and experimental values. The issue of stressbridging due to contact between particles is also explored in the context of GMC. Chapter 6 deals with a realspace renormalization group method for determining the ective properties of composites called the recursive cell method (RCM). Predictions of ective properties from this method for a range of volume fractions and modulus contrasts are compared to estimates from finite element calculations. Estimates of ective elastic properties of models of polymer bonded explosives from the RCM technique are then compared to those from finite element analyses. The RCM technique is also used to explore the percolation behavior of high modulus contrast particulate composites. Finally, some exact relations for the determination of ective properties of composites are discussed in Chapter 7. The predicted ective properties from these exact relations are compared with estimates from finite element calculations, the recursive cell method, and the generalized method of cells. The usefulness of exact relations in determining the accuracy of the three numerical techniques is discussed in the context of high modulus contrast particulate composites.
19 CHAPTER 2 BACKGROUND 2.1 Polymerbonded explosives Polymerbonded explosives (PBXs) are particulate composites containing two or more components. One of the components is an explosive crystal while the other components act as a binder that provides structural support to the crystals. Some PBXs and their components [1, 2, 3] are listed in Table 2.1. It can be observed ( from the table that all these PBXs contain a very high weight fraction of particles 90%). In most cases, at and above room temperature, the particles are considerably stiffer than the binder PBX 9501 The polymerbonded explosive of interest in this research is PBX 9501 because of the availability of experimental data on the mechanical behavior of this material. PBX 9501 is a particulate composite containing crystals of HMX (High Melting Explosive) in a binder composed of Estane 5703 and BDNPA/F. In addition, a free radical inhibitor such as diphenylamine or Irgonox is usually added to the binder [4]. A detailed composition of PBX 9501 is shown in Table 2.2. The small volume fraction occupied by Irgonox can be neglected. The voids occupy only 2% of the volume and are neglected in this research Elastic properties of PBX 9501 The elastic moduli of polymer bonded explosives are strongly influenced by strain rate and temperature [7] because of the strain rate and temperature dependent behavior of the binder. In general, the compressive strengths and elastic modulus of polymerbonded explosives increase with decreasing temperature and increasing strain rate. The above observations are also true for PBX Temperature and strain rate dependent moduli of PBX 9501 reported by Wetzel [8] and obtained from experiments performed by Wiegand [9], Dick et al. [5], and Gray et
20 5 Table 2.1. Compositions of common PBX materials. Binder Type PBX Explosive/Binder Weight (%) Source Fluoropolymer LX101 HMX a /Viton b 95.5/4.5 [1] (e.g., Viton) PBX 9502 TATB c /KELF800 d 95/5 [1] PBX 9010 RDX e /KELF3700 f 90/10 [2] PBX 9407 RDX/Exon461 g 94/6 [2] PBX 9207 HMX/Exon /8 [2] Polyeurethene PBX 9011 HMX/Estane 5703 h 90/10 [2] EDC 29 HMX/HTPB i 95/5 [3] Polyeurethene PBX 9404 HMX/NC j +CEF k (1:1) 94/6 [2] (with EDC 37 HMX/NC+K10 l (1:8) 91/9 [3] Plasticizers) PBX 9501 HMX/ 95/5 [2] Estane 5703+BDNPA/F m (1:1) a HMX : 1,3,5,7tetranitro1,3,5,7tetraazacyclooctane b Viton : random copolymer of hexfluoropropane and vinylidene fluoride (1:2) c TATB : triaminotrinitrobenzene d KELF800 : random copolymer of chlorotrifluoroethylene and vinylidene fluoride (3:1) C H N O e RDX : f KELF3700 : (CFClCF CH CF ) g Exon461 : (CFClCF CH CF ) h Estane 5703 : segmented polyeurethene of low molecular weight poly(butylene adipate) soft segments and 4,4 diphenylmethane diisocyanate 1,4 butanediol hard segments. i HTPB : hydroxyl terminated poly butadiene j NC : nitrocellulose k CEF : chloroethyl phosphate l K10 : plasticizer (composition not known) m BDNPA/F : bisdinitropropylacetal/formal Table 2.2. Weight and volume fractions of the components of PBX Component Weight Volume Fraction Fraction a HMX b Estane BDNPA/F Irgonox Voids a The volume fraction data have been obtained from Dick et al. [5]. b McAfee et al. [6] cite volume fractions of and for HMX and binder respectively.
21 6 al. [4] are shown in Figure 2.1. The high strain rate Young s modulus is around 12 times the low strain rate Young s modulus at room temperature. The Poisson s ratio of PBX 9501 is around 0.35 at room temperature. No data on the coicient of thermal expansion of PBX 9501 have been found in the literature Particles  HMX ( HMX crystals can exist in three stable phases HMX, HMX, and HMX) depending on temperature and pressure. Data obtained by Leiber [10] on these phases and their ranges of stability are shown in Table 2.3. The HMX phase is dominant at or near room temperature when linear elastic behavior is expected HMX crystal structure is the axis of secondorder symmetry (or equivalently the plane  is the plane of The HMX crystal has a monoclinic structure as shown in Figure 2.2. The axis symmetry). At room temperature the lattice parameters, ratio! "$#&% '(')%+*,"# and are approximately in the and the angle is approximately.0/21 (Bedrov et al. [11]). Young s Modulus (GPa) o C 40 o C 27 o C 25 o C 17 o C 0 o C 20 o C 40 o C 55 o C Young s Modulus (GPa) /s 0.01/s 0.05/s 0.11/s 0.44/s 2250/s (/s) Strain Rate (a) Temperature ( o C) (b) Figure 2.1. Young s modulus of PBX 9501 (a) as a function of strain rate (b) as a function of temperature.
22 7 Table 2.3. Different phases of HMX and transition temperatures. Phase Stable (3 Region Transitions C) 4 ( ( HMX ) at 1163 C 9 ( HMX ) at C HMX 162melt ) at C c β a b a = b = c o α = γ = 90 = β Figure 2.2. Monoclinic structure of a7 HMX crystal.
23 Elastic moduli of: HMX Crystals of: HMX behave in a mildly nonlinear elastic manner at ambient temperatures. With increase in temperature, voids develop in the crystals that lead to considerable degradation of elastic stiffness before melting. However, a linear elastic approximation is adequate for: HMX below 40; C. The elastic constitutive relation for a monoclinic HMX crystal is shown in equation (2.1) [12] where the< axis in Figure 2.2 (also referred to as the 2 axis [13]) is the axis of second order HJIIIIII KML >>>>>>=? N ACA N AGD N AGE O N N AGP O AGD N DCD N DCE O N N DCP O AGE N DCE N ECE O N ECP O O O O NRQCQ O NRQTS N AGP N DCP N ECP O N PCP O O O O NRQTS O NUSCS HJIIIIII K >>>>>>=? VWACA VFDCD VFECE VFDCE VFEFA VWAGD HJIIIIII K (2.1) Linear elastic moduli of: HMX have been determined experimentally by Zaug [14] and Dick et al. [5] from measurements of wave velocities through single crystals. Molecular dynamics (MD) simulations by Sewell et al. [15] have also been used to estimate the stiffness matrix of: HMX. The stiffness matrix of: HMX from experiments and MD simulations is shown in Table 2.4. The values of the 13 elastic coicients shown in the table were calculated by Zaug at a temperature of 107; C using a nonlinear least squares simplex fit of the experimental data using the room temperature value of bulk modulus (12.5 GPa) as a benchmark. The molecular dynamics simulations by Sewell et al. (shown inside round brackets in Table 2.4) are observed to be quite close to the experimental values Thermal expansion of: HMX The coicients of thermal expansion (CTEs) of HMX crystals shown in Table 2.5 have been determined both from Xray diffraction experiments [16] and from MD simulations [11]. The values show a pronounced anisotropy in the< lattice direction compared to thex andy directions. Although the anglesz (between thex and< lattice directions) and[ (between thex andy lattice directions) do not vary significantly with temperature, there is a large change in the angle: of the monoclinic lattice.
24 9 Table 2.4. The stiffness matrix of\ HMX [14, 15]. All values are in GPa. Numbers inside round brackets are from MD simulations [15] (18.7) 3.9 (4.9) 12.5 (7.7) (1.7) (17.0) 6.5 (7.3) (3.0) (16.7) (0.2) (8.9) (2.4) Symm. 6.4 (9.3) (9.8) Table 2.5. Thermal expansion properties of\ HMX. Expts. (]_^a`+b+c /K) MD (]d^a`+b+c /K) \ (Herrmann [16]) (Bedrov et al.[11]) Lattice Parameters a Linear/Angular b Expansion c Volume Expansion
25 Particle size distribution in PBX 9501 The dry blend of HMX particles in PBX 9501 is a mixture of two different size distributions of particles. The coarse HMX particles are sized between 44 and 300 microns while the fine particles are less than 44 microns in size. The particles are mixed in a 3 to 1 ratio of coarse to fine particles. In the composite, the smaller particles fit into the interstitial spaces between the larger ones. The large particles occupy most of the volume of the composite. A particle distribution for the dry blend is shown in Table 2.6. The manufacture of PBX 9501 involves mixing the dry blend of HMX and the binder to form molding powder granules (prills) of PBX These powders are then isostatically compressed at 90e C until the porosity is reduced to 12% and the pressed form of PBX 9501 is obtained. The size distribution of HMX particles in PBX 9501 after processing is significantly different from that before processing. Experiments by Skidmore et al. [17] have shown that the cumulative volume fraction of the finer sized particles is dramatically higher in pressed PBX 9501 compared to the dry blend. Figure 2.3 shows the particle size distributions of HMX in the dry blend and in pressed PBX Experiments by Skidmore et al. [18] have shown that the consolidation of prills initially involves little damage to the large HMX crystals. As porosity is decreased, there is an increasing incidence of transgranular cracking and twinning in the large HMX crystals. If porosity is decreased to less that 1%, microcracks grow across crystals due to crystaltocrystal contact and intercrystalline indentation Binder  Estane 5703 and BDNPA/F The binder in PBX 9501 is essentially a combination of Estane 5703 and a plasticizer (BDNPAF). A free radical inhibitor (Irgonox) is added for further stability of PBX Estane 5703 is amorphous and thermoplastic with a relatively low glass transition temperature (31e C) and a melting temperature of around 105e C. It contains soft and hard segments that serve to enhance entanglement and leads to low temperature flexibility, high temperature stability and good adhesive properties. The plasticizer (BDNPA/F) decreases the binder strength and stiffness.
26 11 Table 2.6. HMX particle size distributions in the PBX 9501 dry blend [8]. Particle f Size Coarse HMX Fine HMX (microns) f (Wt. %) (Wt. %) f % at least 75% f % f 125 at least 98% % 100% % 12 PBX 9501 Dry Blend Pressed PBX 9501 Volume Fraction (%) Particle Diameter (microns) Figure 2.3. HMX particle size distributions in PBX 9501 at various stages of processing (adapted from [17]).
27 Elastic moduli of PBX 9501 binder The elastic properties of the PBX 9501 binder are sensitive to strain rate and temperature. Binder moduli are difficult to determine experimentally because of the low stiffness of the material. Moduli from MD simulations of the binder constituents are not yet available. Approximate elastic moduli of the PBX 9501 binder from experiments performed by Dick et al. [5], Cady et al. [7, 19], Gray et al. [4] and Wetzel [8] at various strain rates and temperatures are shown in Figure 2.4. The Young s modulus of the binder shows considerable scatter at high strain rates. The Poisson s ratio of the binder is close to 0.5, as can be expected of rubbers and elastomers Thermal expansion of PBX 9501 binder Wetzel [8] cites the coicient of thermal expansion of Estane 5703 to be between 10g_hai+j+k to 20gdhai+j+k /K. Since data are not available for the binder, the coicient of thermal expansion of the PBX 9501 binder is assumed to be the same as that of Estane Young s Modulus (GPa) o C 22 o C 16 o C 0 o C 15 o C 20 o C 40 o C Young s Modulus (GPa) /s 0.005/s 0.008/s 0.034/s 0.049/s 1/s 1000/s 1200/s 1300/s 1700/s 2200/s 2400/s 10 1 (/s) Strain Rate (a) Temperature ( o C) (b) Figure 2.4. Young s modulus of PBX 9501 binder (a) as a function of strain rate (b) as a function of temperature.
28 Mock polymerbonded explosives Mock polymer bonded explosives containing glass beads or sugar instead of explosive particles have also been studied by various researchers [7, 8]. These mock materials can be easily tested in the laboratory and can be used to validate micromechanics methods for the prediction of ective properties of polymer bonded explosives. 2.2 Micromechanics of composites The term micromechanics describes a class of methods for determining the ective material properties of composites given the material properties of the constituents. In these methods, governing equations based on continuum approximations are used to determine ective properties. The material properties of interest in this work are the linear elastic moduli and coicients of thermal expansion of PBXs. The high volume fraction of the dispersed component in PBXs as well as the high modulus contrast between the dispersed and the continuous components provide the main challenges. In this section, some rigorous bounds and analytical approximations for ective moduli are reviewed and the ectiveness of these methods is discussed in the context of PBX 9501 at room temperature and under low strain rates. In addition, numerical methods of calculating ective properties are also reviewed Rigorous bounds The most elementary rigorous bounds on elastic moduli are the Voigt (arithmetic mean) and Reuss (harmonic mean) bounds [20] which can be written as l6mnpol6qsrutvmnwotxqbr Voigt Bounds (2.2) y{z l npoy{z l6qsr y{z t} npo y{z tvqr Reuss Bounds (2.3) ~ o~ q n ~ ƒ ~ C r { where, for a quantity, ; are particle and binder volume fractions;l rˆl rˆl are particle, binder and composite bulk moduli; andt rˆt rˆt are particle, binder and composite shear moduli. The superscipts andš denote upper and lower bounds on an ective property.
29 ½ HashinShtrikman bounds Variational principles based on the concept of a polarization field have been used by Hashin and Shtrikman [21] to obtain improved bounds on the ective elastic moduli that have been shown to be optimal for assemblages of coated spheres. For particulate composites these bounds can be written as 6Œ pž 6 u ( W š š œ Ž 6 ˆ Ÿž2 HashinShtrikman Upper Bounds (2.4) Œ pžx 2 { W Ÿ T œžv ˆ (2.5) { ª pž { 6 ž W a { { T ž «6 ˆ HashinShtrikman Lower Bounds (2.6) { ª pž { v u W { ä C Ž«{ v (2.7) Ž š W ; and ³²µ M 0 0 ³ ² Ÿž2 ¹ ( º ¼» (2.8) where, for a quantity, ± Bounds on the ective coicient of thermal expansion of a twocomponent isotropic composite can be calculated using the HashinShtrikman bounds [22]. These bounds are ½ Œ pž½ ¾ ž W a Ÿ ½ ½ { ¹ž2 Ž 6 RosenHashin Upper Bound (2.9) ½ ª pž½ ¾ ž W a ½ ½ ¹ž2 Ž 6 RosenHashin Lower Bound (2.10) ½ ½ where are the coicients of thermal expansion of particles, binder and composite, respectively Thirdorder bounds Thirdorder bounds [23] improve upon the HashinShtrikman bounds by using threepoint correlation functions [24, 25] to incorporate geometric information into the de
30 15 termination of upper and lower bounds on ective properties. These bounds can be expressed as À6ÁÂpÃÀ6Ä Å Æ2Ç È Ç É ÊÀ È Å À ÉšËTÌ ÆÍ ÃÀ6Ä ÎŸÏ ÃGÐ ÄTÑ Ò Thirdorder Upper Bounds (2.11) Ð ÁÂpÃÓÐ Ä Å Ô2ÇWÈ{Ç{ÉWÊÐ È Å Ð ÉTËTÌ Ô ÍÃÓÐ ÄˆÎ Õ Ò (2.12) Öa ÀØÂpÃÖ{ À6ÄuÅ Ï ÇWÈ{Ç{ÉBÊÖ{ À È Å Öa À Ï Ù ÉTËÌ ÃÖa À6ÄˆÎ Æ ÃÖ{ Ð ÄTÑ Ò Thirdorder Lower Bounds (2.13) Ö{ Ð ØÂpÃÖ{ Ä Å Ç È Ç ÉÊÖ{ Ð Ð È Å Ö{ Ù Ð ÉTËÌ Ã Ö{ Ð Ä Î Ô(Ú Ò (2.14) where, for a quantityû,ãû ÄFÑ Â Û ÈaÜÝÈ Î Û ÉCÜWÉ, andãû ÄšÞ Â Û ÈaßàÈ Î Û Éáß0É Öºâ ÃÀ6Ä. Also, Ú Â Ì ÃÖ{ À6ÄÝÑ ÎMã ÃÓÐ Ä ÃÆ Ð ÎMä0À6Ä Ã Ö{ Ð ÄšÑåÎ ÃÆ ÀæÎ Ð ÄÌ Ã Ö{ Ð ÄTÞ Ãèç ÀæÎ¹é Ð ÄÌ Ò (2.15) Õ Öºâ Â ÃGÐ ÄÌ ÃÀ6ÄÝÑåÎ ã ÃÓÐ Ä ÃÆ Ð ÎMä0À6Ä ÃèÐ ÄÝÑåÎ ÃÆ ÀæÎ Ð Ä Ì ÃèÐ ÄšÞ ÃÀêÎ ä Ð Ä Ì ë (2.16) These bounds depend on two extra geometric parameters,ü È Â Ö Å ÜàÉ andß È Â Ö Å ß É which incorporate the threepoint correlation functions and have been found to lie between 0 and 1. If the assumption is made that the penetrable spheres model (where spheres placed randomly in the RVE may overlap) is representative of high volume fraction particulate composites, the values of ÜìÈ and ß È listed by Berryman [26] can be extrapolated to a volume fraction of 0.92 to obtainü È = andßºè = These values have been used to calculate thirdorder bounds for PBX Comparison of bounds Table 2.7 shows the data used to compute the VoigtReuss, HashinShtrikman and thirdorder bounds for PBX 9501 shown in Table 2.8. The elastic moduli of HMX in Table 2.7 are based on bounds provided by Zaug [14]. The elastic moduli of the binder and PBX 9501 are based on an average of the low strain rate data. The coicients of thermal expansion are from Bedrov et al. [11]. The thirdorder bounds in Table 2.8 provide the best estimates of the elastic moduli of PBX 9501 of the three. Lower bounds are closer to the experimental data than upper
31 16 Table 2.7. Elastic moduli and CTE of PBX 9501 and its components at room temperature and low strain rate. Material Volume Young s Poisson s Bulk Shear CTE Fraction Modulus Ratio Modulus Modulus (%) (MPa) (MPa) (MPa) (10í+î /K) HMX Binder PBX Table 2.8. Bounds on properties of PBX Bulk Modulus Shear Modulus Thermal Expansion (MPa) (MPa) (ï_ðañ í+î /K) Upper Bounds Voigt HashinShtrikman Thirdorder PBX 9501 (Experiments) Lower Bounds Thirdorder HashinShtrikman Reuss bounds. The best lower bound predicts ective bulk and shear moduli that are about 20% of the bulk and shear moduli of PBX This implies that accurate estimates of the ective elastic moduli of PBXs cannot be obtained from rigorous bounds at low strain rates and ambient temperature. On the other hand, the bounds on the coicient of thermal expansion of PBX 9501 are within 6% of each other. Therefore, these bounds can be used to estimate the CTEs of some PBXs Analytical methods Analytical methods for approximating ective elastic moduli of random composites have been developed by researchers since the early 1900s. Early developments were based on dilute dispersions of particles in a continuous matrix assuming that there were no particleparticle interactions. More recent developments have explored concentrated
32 ó 17 dispersions where particleparticle interactions are allowed. For high volume fraction particulate composites, the composite spheres assemblage, selfconsistent schemes, and the differential ective medium approach are of interest. The ective CTE of an isotropic composite containing isotropic components can be determined exactly, provided the ective bulk modulus of the composite is known, using the expression [22] ò ópôò õåöÿ }øa úùdû ò øüöÿòˆù }øüöÿ ùáýÿþ ö ô 6õ (2.17) Composite spheres assemblage (CSA) The composite spheres assemblage model [27] idealizes a particulate composite with spherical particles coated by a layer of binder. The volume of the composite is assumed to be filled completely with various sizes of these coated spheres. The ratio of the radius of a spherical particle to the thickness of its coating reflects the volume fraction of particles in the composite. The solution of the problem involves placing a coated sphere in the ective medium and applying a hydrostatic stress at the boundary of the coated sphere. This approach leads to an expression for the ective bulk modulus that can be written as ù Wøúû }ødöÿ ù ù úù ùáý (2.18) Expressions for the ective shear modulus from the CSA model are available that are valid in the limit of low particle volume fraction (the dilute approximation). However, for high concentrations of particles, the shear modulus cannot be found accurately using the CSA model Selfconsistent schemes (SCS) The ective stiffness tensor of a dilute distribution of particles in a continuous binder can be expressed as [28] where ø ù! ó ù Wø þ øxö ù þ ø ù þ Wø (2.19) are the stiffness tensors of the particles, binder, and composite, and is the tensor that relates the applied strain to the strain in a particle. When the volume
33 " * E * E [ A $ & I & A K A A $ 8 8? 18 fractions of particles is more than 5%, the binder in the dilute approximation is replaced with a material that possesses the unknown ective elastic properties of the composite. Thus, the expression for the ective stiffness tensor is changed to # "%$'&()+*,")./"%$103245*6"7) 89" 0:&;<*=(>)!0? (2.20) The above equation can be solved for the ective stiffness of the composite for various particle shapes. This procedure is called the selfconsistent scheme, the ective medium approximation and also the coherent potential approximation. Various types of selfconsistent approximations of ective composite properties can be found in the literature [29, 30]. For a particulate composite containing a dispersion of elastic spheres, the commonly used selfconsistent scheme leads to the following equations and A that are solved # # $B&()DC AQ$B&() C E AR)LSAN$ &HG &JA &U G V E!X Differential ective medium approach (DEM) K K )F )L KNM'OP AR)FYA AR)F/AQ$ KZM OP (2.21) (2.22) The differential ective medium approach has been successfully applied to approximate the ective properties of composites containing particles in a continuous binder, mostly for low volume fractions of particles [28, 29, 31]. In this approach, an infinitesimal volume of particles is added to the binder and the ective properties are calculated using a dilute approximation. The binder is then replaced by the ective material, an infinitesimal volume of particles added, and the ective properties calculated. This process is repeated until the actual volume fraction of particles is obtained. This approach can be represented by the following coupled system of linear first order ordinary differential equations that can be solved using a fourthorder RungeKutta scheme. () # (>)0\[ () # )L *,AL)LSA &J 0 V I )]&J V I &^ 0 G K (2.23) (2.24)
34 d g b b where _a`cb efg hi hj kml Several other approximation schemes exist that generate analytical equations relating the ective elastic moduli to the constituent moduli and volume fractions. Details of these approaches can be found in the monograph by Milton [32] Comparison of analytical approaches Estimates of the ective properties of PBX 9501 using analytical approaches are shown in Table 2.9. The properties of the components of PBX 9501 listed in Table 2.7 have been used in these calculations. The bulk modulus estimate from the composite spheres assemblage approach matches the lower bound predicted by the Hashin Shtrikman bounds and is considerably lower than the experimentally determined bulk modulus. The values of the bulk and shear modulus predicted by the selfconsistent scheme are about 10 times the experimental values. The differential ective medium estimates are improvements over the thirdorder bounds discussed before. These estimates are still considerably lower than the experimentally determined moduli. The estimates of CTE depend on the accuracy of the estimates of bulk modulus. However, for PBX 9501, the low CTE contrast of the two components leads to approximately the same value of ective CTE. In fact, considering the large modulus contrast between the particle and the binder, the differential ective medium estimates are quite accurate and can be used when no better approximations are available. Table 2.9. Analytical estimates of properties of PBX Bulk Modulus Shear Modulus Thermal Expansion (MPa) (MPa) ( nro!p+q+r /K) Composite Spheres Selfconsistent Scheme Diff. Effective Medium Experiments
35 Numerical approximations The ective elastic moduli of a particulate composite can be determined approximately by determining the stresses and strains in a representative volume element under appropriate boundary conditions using numerical methods. The ective stiffness tensor s tvu w9x of the composite can then be obtained from the relation y6z tvu1{} ~ s t u w9x y= w}x { (2.25) where y6z tvu1{ are the volume averaged stresses and y= t uƒ{ are the volume averaged strains. The earliest numerical approximations of ective elastic moduli were carried out using finite difference schemes [33, 34]. These were twodimensional approximations for regular arrays of fibers in a matrix. Randomly generated microstructures in two dimensions were simulated soon after these preliminary investigations [35]. More recently, researchers have approached this problem using finite element methods [36, 37], boundary integral methods [38, 39, 40], Fourier transform based methods [41, 42], and the method of cells [43]. Threedimensional simulations are also increasingly being carried out [44, 45] The representative volume element The representative volume element (RVE) is conceptually similar to the crystallographic unit cell which is the building block in the structure of crystals [46]. Indeed, unit cells are the most commonly used RVEs. The size of the RVE and the amount of geometrical detail modeled has been determined primarily by the availability of computational power. Though Sab [47] has shown that the ective properties of a random composite can be calculated by the simulation of one single RVE, this single RVE is not easy to determine. A more practical approach is to simulate a large number of smaller RVEs so that some statistics on the ective properties are obtained. For a composite containing randomly distributed monodisperse spheres, the RVE size is about two sphere diameters [48] if only ective elastic properties are required. However, such rules of thumb are not available for other types of random particulate composites. In twodimensional studies, the microstructure of particulate composites has been modeled with monodisperse circular particles [49], square particles [50], and arbitrarily
36 21 shaped particles [51]. The particles have been placed in a random sequential manner in the RVE in all these studies. Twodimensional models of PBXs have also used circular and square particles distributed using a molecular dynamics based approach [52]. Some attempts have also been made to create RVEs from digitized micrographs of PBXs [53]. Most studies of particulate composites deal with twodimensional microstructures. However, a few threedimensional studies have also been performed [54, 44, 55]. A commonly used procedure for threedimensional microstructure generation is random sequential placement of spherical/cubical particles in a RVE. This approach is not suitable for high volume fraction composites like PBX 9501 because sequential placement of particles becomes extremely inicient beyond volume fractions of 45%. The molecular dynamics based approach of Baer [52] is an improvement over sequential placement. However, locking of particles leads to maximum achievable volume fractions of around 70%. A more practicable approach, for PBXlike materials, is the digital image processing based method adopted by Garbozci and Day [54]. In this method, Xray tomography is used to generate threedimensional voxelized images of the composite. Terada et al. [55] have also developed detailed digital image based models of composites that use twodimensional slices to generate threedimensional microstructures. Though digital techniques appear lucrative, advanced image processing techniques are required to generate microstructures for PBX 9501 because the high volume fractions and similar densities and reflectivities of particles and binder make it difficult to identify the components of the composite from images Finite element approximations Random particulate composites containing low volume fractions of particles can be approximated by square arrays of fibers in two dimensions [49] and cubic arrays of spheres in three dimensions [36]. Displacement based finite element solutions have been found to predict ective properties that overestimate the actual properties while forcebased solutions provide a lower bound on the actual properties. A recent study, performed on regular arrays of fibers by Pecullan et al. [56], has found that the force based ective stiffness tensor is more accurate for a composite with high modulus contrast and
37 22 a compliant matrix. Force based finite element methods are not utilized in this research because of the difficulties in formulation and implementation of these methods. The multiphase finite element method [57] is a variation of the standard displacementbased finite element approach. In this method, different material properties are assigned to different Gauss points in the finite element analysis of a complex microstructure. This approximation eliminates the need to generate complex meshes to describe the geometry. However, the robustness of the method is still not very well established. Ramakrishnan et al. [51] have used a generalized plane strain approach to model particulate metal matrix composites where particles of various shapes and sizes were randomly distributed in a twodimensional square RVE. The ective Young s modulus was determined by the application of a uniform unidirectional displacement. The ective bulk modulus was determined by applying equal displacements in the three orthogonal directions. It is observed that the shapes of the particles do not have any significant ect on the ective elastic properties even though many particles have sharp acute angles and therefore high stress concentrations. Random distributions of particles in two dimensions have also been studied by Theocaris et al. [58] in the context of determining the ective Poisson s ratio. Finite element simulations were performed on a unit cell with periodic boundary conditions and uniform prestresses. The ective elastic properties were determined using a strain energy match between a cell simulating the microstructure and an equivalent homogeneous cell. This study shows that Poisson s ratios calculated using twodimensional models are actually twodimensional Poisson s ratios that have an upper bound of 1.0 instead of the 0.5 for the threedimensional case. The study also suggests that sharp corners in particles do not have any significant ect on the ective elastic properties  assuming perfect interfacial bonding. A twostep approach has been used by Jia and Povirk [50] to model a twophase composite containing randomly distributed square inclusions. In this approach, a window of the RVE is chosen in the first stage of the calculations and moved over the RVE. Twodimensional displacement based finite elements are used to calculate the ective properties at each location of the window. These ective properties are then assigned
38 23 to a smaller mesh for faster calculations of the overall properties. The study finds that the error in the estimation is small for the component properties considered. Pecullan et al. [56] have also observed that replacement of the smallest scale microstructure by the equivalent homogeneous material does not cause large errors in calculation of the ective stiffness tensors. This result is of interest in this research because generation of microstructures occupying more that 86% of the volume is difficult. Instead, we can generate microstructures that occupy about 86% of the volume and replace the remaining volume with a dirty binder (a binder with the ective properties of a mixture of particles and the original binder) without much loss in accuracy. In the threedimensional study by Gusev [44], RVEs containing spheres have been modeled using displacementbased finite elements. The microstructure was discretized using tetrahedral finite elements. This approach is not suitable for high volume fraction composites like PBX 9501 because the meshing of closepacked particles using tetrahedral elements leads to extremely skewed elements and poor numerical accuracy. Finite element meshes are easier to generate from threedimensional voxelized images [54, 55] where each voxel is then modeled as an eightnoded linear displacement finite element. A question that arises for PBXs is whether the binder wets all the particles. In other words, it is of interest to know the amount of strain that leads to interfacial debonding between the particles and the binder. A threedimensional finite element study of the ect of interfaces on the stresses in composites containing spherical inclusions arranged in a cubic array has been carried out by Dong and Wu [59]. The results indicate that the assumption of perfect bonding used in many micromechanics studies may not be appropriate for high concentrations of particles even when small strains are applied because very high interfacial stresses are developed Homogenization theory The mathematical theory of homogenization [60] is an established approach for determining ective properties of periodic composites [61]. In this method, the governing differential equations with rapidly varying coicients are replaced by differential equations with constant or slowly varying coicients. Asymptotic expansions of the field variables along with the assumption of periodicity lead to this transformed set of
39 24 equations. The modified problem, called the Yperiodic homogenization problem, is then solved using finite elements or other techniques. Ghosh and coworkers [62, 37] have used homogenization theory along with the Voronoi cell finite element method to model RVEs containing random distributions of particles at volume fractions of up to 50%. In this approach, particle locations are generated within the RVE using a random process. A weighted Voronoi tessellation of these particles is carried out to generate a set of Voronoi cells each containing a single particle. Homogenization theory is used to model the ect of a single particle on the properties of a Voronoi cell. The approach shows good agreement with detailed finite element analyses of the same microstructure. However, for high particle volume fractions ( 80%) a weighted Voronoi tessellation can lead to needle shaped cells in two dimensions. In three dimensions, generation of weighted Voronoi tessellations is considerably involved. These considerations make this approach unsuitable for high volume fraction particulate composites Stochastic finite elements In continuum descriptions of composites, the constitutive relationship is only a function of spatial position. Stochastic descriptions of the constitutive relation assume that the stiffness tensor is a random field with continuous realizations. In other words, an additional stochastic variable is added to the continuum description. Stochastic finite element analyses attempt to solve this modified problem using finite element techniques. These methods are applicable to particulate composites where the particle distributions can vary in a random manner. OstojaStarzewski [63] has performed stochastic finite element analyses on twodimensional composites reinforced by randomly located disks. Numerous simulations have been carried out to obtain bounds on the ective stiffness tensor. These analyses show, for a given RVE size, that the predicted bounds deviate from each other by 0.5% as the modulus contrast between the components reaches about 20. Huyse and Maes [64] have used stochastic finite element analyses (using a truss network to represent a particulate composite) to determine the autocorrelation and crosscorrelation coicients between various elastic constants. OstojaStarzewski [65] has suggested that
40 25 these correlation coicients could be easily determined for particulate composites. This information could be then be used to generate bounds on the ective elastic response without resorting to time consuming numerical simulations of different realizations of the microstructure Discrete models Discrete models, e.g., spring network models, are receiving renewed attention because they are easier to generate and faster to solve. Twodimensional triangular spring network models have been used by Day et al. [66] to determine the ective elastic response of plates containing randomly located holes. Toi and Kiyoshe [67] used a three dimensional discrete model consisting of springs and rigid crystals to determine the ective mechanical properties of polycrystals with damage. Network based approximations for high contrast, high volume fraction composites have also been developed by Berlyand and Kolpakov [68]. These models generate quite accurate results. Voronoi tessellations of the geometry are required in some of these models and the associated problems of generating these tessellations for high volume fraction materials make these models unattractive for PBXs. On the other hand, digital images of random composites can easily be resolved into spring networks though some involved image processing is necessary to obtain suitable images of PBXs Integral equation methods Boundary integral based methods have been used with some success for determining the ective mechanical and thermal properties of twodimensional composites (e.g., Rizzo and Shippy [38], Achenbach and Zhu [39], Papathanasiou et al. [69], Helsing [70, 71]). The computations of Rizzo and Shippy [38] for square inclusions avoided calculations of stresses at the corner singularity regions. The calculations of Achenbach and Zhu [39] were carried out on single circular inclusions using standard boundary element techniques. Similar methods have been used to determine the ective elastic moduli of twodimensional composites with low volume fractions of circular inclusions by Papathanasiou et al. [69]. The interface integral method of Helsing [71, 72] has been used to generate accurate
41 26 ective elastic properties of periodic composites in two dimensions. An Airy stress function based complex variable representation of the governing differential equation is converted into the ShermanLauricella type integral equation in this technique. The integral equation is solved using a matrix free Nyström algorithm [71]. The Helsing method has been used to determine accurate ective elastic moduli of RVEs containing large numbers of complex shaped inclusions nearly in contact [73]. This technique promises to be one of the best available for twodimensional analysis of the low strain rate micromechanics of composites. It is especially suited for problems that involve stress singularities. The use of complex variables leads to the method being applicable only to twodimensional problems in its current form. If the particles touch each other or have high modulus contrast, convergence is reported to be relatively slow. The implementation of the Nyström algorithm consists of several steps and is quite involved, making this method unattractive for this research Fourier transform method Complex microstructures have also been studied by Moulinec and Suquet [41] using a Fourier transform based numerical approach to solve the unit cell problem. This approach takes advantage of the assumed periodicity of the elastic fields and by reducing the governing differential equations to the LippmanSchwinger equation form both in real space and Fourier space. The solution is then obtained using an explicit algorithm that alternates between the real and the Fourier spaces. Discretization of the problem is carried out using a regular grid of pixels or voxels generated from images of microstructures. The advantage of this method is that special consideration is not required for materials that are nearly incompressible (as is needed to avoid element locking in finite element approaches). However, for high modulus contrast between the components, the rate of convergence is slow. This problem has been partially solved using an accelerated convergence method [42, 74] that converges as the square root of the modulus contrast. The Fourier transform based method is attractive because it can easily be extended to model threedimensional problems and inelastic material behavior in PBXs.
42 Generalized method of cells The generalized method of cells (GMC) [43, 75] has been used to model the micromechanical behavior of different types of composites with relative success. The advantage of this method over other numerical techniques is that the full set of ective elastic properties can be calculated in one step instead of solving a number of boundary value problems with different boundary conditions. The problem of discretization is also minimized because a regular rectangular grid is used. GMC uses an averaging technique that satisfies subcell continuity and equilibrium in an average sense using integrals over subcell boundaries. This method has been shown to be more computationally icient than finite elements for modeling fiber composites [76]. However, the computational iciency of GMC decreases and can become worse than that of finite elements as the number of subcells increases because the size of the matrix that is inverted is the square/cube of the number of subcells in two/three dimensions. This leads to large memory requirements and large computational times while modeling complex microstructures. The computational iciency of GMC has been improved after reformulation by Pindera and Bednarcyk [77, 78, 79, 80]. The reformulation has taken advantage of the continuity of tractions across subcells to obtain a system of < 6 ˆ Š equations in three dimensions. There is a lack of coupling between the normal and shear stresses and strains in GMC. Bednarcyk and Arnold [81] claim that this lack of coupling makes for an ultraicient micromechanics model. However, this lack of coupling leads to the gross underestimation of shear moduli. Recently, Williams and Aboudi [82] have attempted to rectify the shearcoupling problem for periodic arrays of fibers using a third order expansion for the displacement field. However, this approach leads to a large system of equations and the iciencies introduced by Pindera and Bednarcyk are no longer applicable. An alternative approach has been taken by Gan et al. [83] to include normalshear coupling in the GMC analysis. The original GMC assumes that there is traction continuity across all cell and subcell interfaces. The modification made by Gan et al. removes this constraint and instead attempts to satisfy subcell equilibrium and compatibility. Results obtained by the new method show a much better prediction of shear moduli than the original GMC.
43 CHAPTER 3 MICROMECHANICS SIMULATIONS OF GLASSESTANE MOCK POLYMER BONDED EXPLOSIVES 3.1 Abstract Polymer bonded explosives (PBXs) are particulate composites containing explosive particles and a continuous binder. The explosive particles occupy high volume fractions, often greater than 90%. Additionally, the elastic modulus of the particles, at room temperature and higher, is often three to four orders of magnitude higher than that of the binder. Both experimental and numerical determination of macroscopic properties of these composites is difficult. High modulus contrast mock polymer bonded explosives provide a means of relatively inexpensive experimentation and validation of numerical approaches to determine properties of these materials. The goal of this investigation is to determine whether the ective elastic properties of monodisperse glassestane mock polymer bonded explosives can be predicted from twodimensional micromechanics simulations using the finite element method. In this study, the ect of representative volume element size on the prediction of twodimensional properties is explored. Twodimensional estimates of elastic properties are compared with predictions from threedimensional computations and with experimental data on glassestane composites containing three different volume fractions of spherical glass beads. The ect of particle debonding on the ective elastic properties is also investigated using contact analyses. Results show that twodimensional unit cells containing 10 to 20 circular particles are adequate for modeling glassestane composites containing less than 60% glass particles by volume. No significant difference is observed between properties predicted by the two and threedimensional models. Finite element simulations of
44 29 representative volume elements, containing particles that are perfectly bonded to the binder, produce estimates of Young s modulus that are higher than the experimental data. Incorporation of debonding between particles and the binder causes the ective Young s modulus to decrease. However, the predicted values of Young s modulus, in the presence of debonding, are still higher than experimental data suggesting that there is considerable debonding between particles and the binder in mock polymer bonder explosives composed of glass and estane. These results indicate the twodimensional finite element simulations that incorporate some amount of damage can be used to obtain accurate estimates of the ective properties of glassestane composites and possibly of polymer bonded explosives with high modulus contrast. 3.2 Introduction Polymer bonded explosives (PBXs) are extensively used as propellants in solid rocket motors. These materials are typically viscoelastic particulate composites containing high volume fractions of explosive particles suspended in a soft binder. For example, PBX 9501 contains about 92% by volume of particles. In addition, the modulus contrast between particles and the binder in PBX 9501 is around 20,000 at room temperature and low strain rates. The high modulus contrast between the particles and the binder as well as the high volume fraction of the particles pose an interesting challenge in the prediction of ective mechanical properties of PBXs using numerical micromechanics techniques. The explosive nature of PBXs makes the experimental determination of their mechanical properties hazardous and thus expensive. Mock polymer bonded explosives containing monodisperse glass beads and an estane binder provide an alternative material that can be tested extensively and used to provide a basis for validating micromechanicsbased predictions of mechanical properties. Since the ects of high particle volume fraction and different particle sizes and shapes do not need to be considered for these glassestane mock explosives, the evaluation of various micromechanics methods is simpler. The validated micromechanics techniques can then be applied to predict the mechanical properties of actual PBXs.
45 30 The goal of this investigation is to determine if the initial moduli of a viscoelastic mock PBX composite can be calculated with reasonable accuracy from the initial moduli of the constituents. The finite element method has been used to estimate the ective elastic moduli of glassestane mock PBXs containing three different volume fractions of glass. First, twodimensional unit cells containing randomly distributed particles are modeled using finite element analysis and the ect of RVE size on the ective properties is investigated. Threedimensional finite element analyses are then performed on selected microstructures to determine if there is a significant difference between twodimensional and threedimensional estimates. The unit cell based estimates are then compared with third order bounds, differential ective medium estimates, and experimental data. Finally, twodimensional simulations of the ect of particle debonding on ective elastic moduli are carried out on a selected microstructure, under both tensile and compressive loading. 3.3 GlassEstane mock PBXs  experimental data The glassestane mock PBXs explored in this investigation are composed of spherical soda lime glass beads (650 Œ 50 microns) contained in an Estane 5703 binder [7]. The glass beads are linear elastic in the range of conditions used in the experiments and have a density of 2.5 gm/cc, a Young s modulus of 50,000 MPa, and a Poisson s ratio of Estane 5703 is an elastomeric rubber with a glass transition temperature of 31 C, a melting point of 105 C and a density of 2 g/cc at room temperature. This polymer contains soft and hard segments that enhance entanglement and lead to low temperature flexibility, high temperature stability and good adhesive properties. The elastic properties of Estane 5703 and the glassestane mocks used in this investigation have been extracted from stressstrain data obtained by Cady et al. [7]. The moduli of Estane 5703 shown in Table 3.1 arare for strain rates of 0.001/s and approximately 2400/s and temperatures ranging from 55 C to 23 C. A Poisson s ratio of 0.49 has been assumed for Estane 5703 under all conditions. The maximum modulus contrast between the glass beads and Estane 5703 is around 10,000. Initial tangent moduli from compression tests on three glassestane composites con
46 31 Table 3.1. Young s modulus of extruded Estane 5703 [7]. Ž Strain Rate = 0.001/s Strain Rate 2400/s Temp. ( C) Modulus (MPa) taining 21%, 44% and 59% by volume of glass (25%, 50% and 65% by weight) are shown in Table 3.2. Cady et al. [7] have observed that at low strain rates, there appears to be good bonding between the glass and the estane binder though there are signs of a few debonded particles. However, at high strain rates the binder shows signs of shear damage and there is some damage in the glass. In this investigation, only the ect of particlebinder debonding is simulated. Fracture of the binder or the glass beads is not considered. 3.4 Estimation of elastic moduli The estimation of ective elastic moduli of a composite using finite elements requires the choice of a unit cell or representative volume element (RVE) that reflects the composition of the composite. The RVE is then subjected to appropriate boundary conditions and the resulting stressstrain field is averaged over the volume of the unit cell. The average stress and strain fields are assumed to obey the relation Table 3.2. Young s modulus of composites containing glass and estane [7]. Ž Strain Rate = 0.001/s Strain Rate 3500/s 21% Glass Temp. ( C) Modulus (MPa) % Glass Temp. ( C) Modulus (MPa) % Glass Temp. ( C) Modulus (MPa)
47 ž Ÿ where is the volume of the unit cell, N v v š9 Zœ š9 are the stresses, œ} v are the strains, and 32 (3.1) the ective stiffness tensor of the composite. The ective stiffness tensor can then be calculated using equation 3.1. An alternative approach for determining the ective orthotropic elastic properties of the unit cell is to compute the boundary forces and displacements produced due to an applied displacement. The twodimensional Young s moduli and Poisson s ratios can then be computed directly using relations such as žrÿ Ÿ \ Ÿ! Ÿ ª! Ÿ where žrÿ is the modulus in the «direction, Ÿ is the Poisson s ratio, force in the «direction, Ÿ is the displacement in the «direction, and v š9 is (3.2) is the reaction is the displacement in the direction. Equations (3.1) and (3.2) have been found to lead to the same twodimensional ective elastic properties. A discussion of two and threedimensional elastic moduli is given in Appendix A. Equations (3.1) and (3.2) give twodimensional elastic moduli for plane strain models. The upper limit on the twodimensional Poisson s ratio is 1.0 [31, 84]. These twodimensional elastic moduli cannot be directly compared with experimentally obtained threedimensional elastic moduli. In this study, the twodimensional ective Young s modulus and Poisson s ratio in the two orthogonal directions are calculated and then averaged to eliminate directional ects. The assumption is made that a planestrain analysis of an isotropic material would lead to these average values. The threedimensional Young s modulus and Poisson s ratio are then calculated using the relations [31] 2D ± 2D ž 2D 6 ³ ² }µ ² (3.3) (3.4) where is the threedimensional Poisson s ratio, ž is the threedimensional Young s modulus, 2D is the twodimensional Poisson s ratio, and ž 2D is the twodimensional Young s modulus. This approach has been found to give estimates of Young s modulus
48 33 and Poisson s ratio that are close to differential ective medium [28] estimates for volume fractions from 0.1 to 0.8 and for modulus contrasts from 10 to 100,000 [85]. 3.5 Twodimensional unit cells The twodimensional unit cell chosen for this study was a square box. Circular particles were placed sequentially into randomly selected positions in the unit cell. A small gap was enforced between adjacent particles so that particleparticle contact would not occur. Particles intersecting the boundary of the unit cell were repeated on opposite boundaries for periodicity of the unit cell. The three glassestane composites (21%, 44%, and 59% by volume of glass) were each modeled using five unit cells of increasing size that contain 5, 10, 20, 50, and 100 particles. Five different particle distributions were generated for each combination of volume fraction and number of particles in the unit cell (25 distributions for each of the three composites). Five particle distributions for each of the three glassestane composites are shown in Figure 3.1. In this study, the finite element analysis package ANSYS [86] was used to simulate the various microstructures. A plane strain assumption was used for the twodimensional analyses. Displacement boundary conditions were applied along one boundary and the nodes along the orthogonal boundary were coupled to move together as shown in Figure 3.2. Periodicity of displacement boundary conditions was enforced along parallel edges of the unit cell. The glass beads (particles) and the estane binder were modeled as isotropic, linear elastic materials. Sixnoded, displacementbased, plane strain triangles were used to discretize the geometry of the twodimensional unit cells used in this study. Bathe [87] has suggested the use of ninenoded mixed displacementpressure (93 u/p) elements to model nearly incompressible materials such as estane. An investigation into the ect of using 93 u/p elements to model the rubbery binder has found that the use of such elements does not significantly affect the ective elastic moduli (compared to moduli obtained using sixnoded displacementbased triangles). A further investigation into the ect of the constitutive law for the binder on the ective properties was
49 34 5 Particles 10 Particles 20 Particles 50 Particles 100 Particles 21% glass 2.8x2.8 mm 2 4x4 mm 2 5.6x5.6 mm 2 8.9x8.9 mm x12.6 mm 2 44% glass 1.9x1.9 mm 2 2.7x2.7 mm 2 3.9x3.9 mm 2 6.1x6.1 mm 2 8.7x8.7 mm 2 59% glass 1.7x1.7 mm 2 2.4x2.4 mm 2 3.4x3.4 mm 2 5.3x5.3 mm 2 7.5x7.5 mm 2 Figure 3.1. Sample particle distributions and unit cells of various sizes containing 21%, 44% and 59% by volume of monodisperse circular particles. Note that the size of the unit cell increases as the number of particles increases Y X Figure 3.2. Displacement boundary conditions used to calculate the stressstrain behavior of a unit cell. A uniform displacement is applied in the direction to nodes 3, 6 and 9. The orthogonal direction displacement at nodes 7, 8 and 9 are coupled so that these nodes move together.
50 35 performed using a plane strain MooneyRivlin rubber model for the estane binder. Nonlinear analyses using the MooneyRivlin rubber model were found to generate stresses and strains similar to those using a linear elastic model. These results suggest that linear elastic displacementbased elements provide a reasonably accurate representation of glassestane composites Effect of unit cell size To determine the ect of unit cell size on the ective elastic properties, twodimensional finite element simulations were performed on particle distributions representing glassestane mock PBXs (as shown in Figure 3.1). The arithmetic mean of the ective Young s modulus and Poisson s ratio has been calculated for five model particle distributions at each combination of volume fraction and unit cell size. Properties of glass and estane at room temperature and at a strain rate of 0.001/s were used in the simulations. Figures 3.3(a) and 3.3(b) show the variation of ective Young s modulus and Poisson s ratio with unit cell size for the glassestane composites with three volume fractions of glass. For the composite containing 21% glass, Figure 3.3(a) shows that the predicted Young s Modulus (MPa) % glass 44% glass 59% glass RVE Size (mm) (a) Young s Modulus. Poisson s Ratio % glass 44% glass 59% glass RVE Size (mm) (b) Poisson s Ratio. Figure 3.3. Variation of ective elastic properties with the size of the unit cell for a strain rate of 0.001/s and at a temperature of 23 C.
51 36 ective Young s modulus is almost constant, both among the five models at a particular unit cell size and between different unit cell sizes. The range of variation of the ective Poisson s ratio, shown in Figure 3.3(b), is also negligible for these particle distributions. For the glassestane composite containing 44% glass, the Young s modulus (Figure 3.3(a)) does not vary much with unit cell size. Variations between different particle distributions at the same unit cell size are also negligible. Though the average ective Poisson s ratio (Figure 3.3(b)) remains relatively constant with unit cell size, there is some variation between particle distributions, especially at smaller unit cell sizes. The ective Young s modulus for a composite containing 59% glass is also shown in Figure 3.3(a). In this case, the mean ective modulus varies slightly for the smaller unit cells. The variation between unit cell sizes becomes negligible for unit cells containing 10 particles or more (¹ 2.4 mm). Additionally, large variations occur between particle distributions for small unit cell sizes. The variation becomes smaller for unit cells containing 50 particles or more (¹ 5 mm). Similar trends are observed for the ective Poisson s ratio shown in Figure 3.3(b). At small unit cell sizes, the variation between particle distributions is large but the mean ective Poisson s ratio stabilizes at unit cell sizes greater than 5 mm. Results shown in Figure 3.3 indicate that the size of the twodimensional unit cell required to calculate the ective properties of monodisperse random composites containing circular particles is quite small. For the three volume fractions investigated, the smallest unit cell that can be used is around 4 mm in size or around six particle diameters. Results in Figure 3.3 also show that the calculation of the ective Poisson s ratio requires a larger unit cell size than that for the ective Young s modulus. A unit cell size of around 5 mm (7.5 particle diameters) is adequate for all the volume fractions modeled. For unit cells containing 21% and 44% by volume of particles, an even smaller unit cell size can be chosen to calculate the ective Poisson s ratio. In general, a unit cell that is 6 to 7 particle diameters in size (or containing 10 to 20 particles) appears to be optimal for the calculation of ective properties of low volume fraction composites containing monodisperse circular particles.
52 3.6 Threedimensional unit cells Twodimensional unit cells were used in this investigation primarily because detailed threedimensional microstructures are difficult to generate and mesh so that they are computationally intensive. The process of generating particle distributions becomes nontrivial for microstructures containing more than 45% by volume of monodisperse spheres. Beyond these concentrations, even if random particle distributions can be generated, the particles are so close to each other that extremely thin elements are required to mesh the regions between particles. Since the number of elements required to discretize threedimensional models is significantly larger than that for corresponding twodimensional models, large computational resources are necessary for threedimensional models. However, comparisons with threedimensional simulations are necessary to determine if twodimensional models adequately represent threedimensional materials such as glassestane composites. To address this issue, twodimensional finite element simulations were compared with threedimensional finite element simulations for unit cells containing 21% and 44% spheres by volume. The threedimensional unit cells were generated such that the length of each side was the same as that for the corresponding twodimensional unit cell containing 10 particles. The unit cells were approximately 4 mm and 2.7 mm in size for the composites containing 21% glass and 44% glass, respectively. The two threedimensional unit cells are shown in Figure 3.4(a). Each of these unit cells was divided into five equal slices using dividing planes perpendicular to one direction. One such slice for each unit cell is shown in Figure 3.4(b). Due to computational limitations, finite element simulations were performed on these slices instead of the complete unit cell. Tennoded tetrahedral elements were used to discretize the geometry of the slices. Displacement boundary conditions similar to those shown in Figure 3.2 were applied to each plane of nodes along the thickness of a slice. Boundary nodes on the plane of the slice were coupled in the out of plane direction. The ective properties of the threedimensional unit cells were calculated using equations (3.1). 37
53 38 21 % Spheres 44 % Spheres (a) Unit cells. 21% Spheres 44% Spheres (b) Slices of the unit cells. Figure 3.4. Threedimensional unit cells containing 21% and 44% by volume of monodisperse circular particles and slices from the unit cells used for threedimensional simulations.
54 39 Figure 3.5(a) shows the ective Young s modulus computed using twodimensional and threedimensional unit cells for 21% glass. Figure 3.5(b) shows the two and threedimensional unit cell based Young s modulus for 44% glass. These estimates are for a strain rate of 0.001/s. The two and threedimensional predictions of Young s modulus do not differ significantly from each other. It is also observed that the threedimensional estimates are always slightly higher than the corresponding twodimensional estimates. The difference between the two and threedimensional estimates is observed to increase with increase in glass volume fraction. Similar results have been obtained for the Poisson s ratio, in which case the difference between two and threedimensional calculations is even smaller. Since the differences between the two are small, the twodimensional finite element calculations are considered sufficiently accurate for the purposes of this work. Two dimensional Three dimensional Two dimensional Three dimensional Young s Modulus (MPa) % glass Temperature ( o C) (a) 21% glass. Young s Modulus (MPa) % glass Temperature ( o C) (b) 44% glass. Figure 3.5. Young s modulus of glassestane composites from twodimensional and threedimensional unit cell based finite element calculations. The estimates are for a strain rate of 0.001/s.
55 Â 3.7 Comparison of estimates and experimental data In this section, ective Young s moduli from twodimensional finite element (FEM) calculations are compared with thirdorder bounds [23] and experimental data. The finite element calculations were performed on unit cells of size approximately 9 mm, 6 mm, and 5 mm for glassestane composites containing 21%, 44%, and 55% glass by volume, respectively (50 particles in each unit cell). The calculation of thirdorder bounds requires knowledge of two geometric parameters º» and ¼ƒ» in addition to the volume fractions ½1» and ½ ¾ of the particles and the binder. For twocomponent composites containing monodisperse nonoverlapping spheres, these parameters are given by [84] 40 º» À Á ÂÄÃÆÅ!ÁÇÈ Á ÂÄÃÆÅ!ÁÇÈ ¼ƒ» ½» Á ÂÕËÌÈÌÃÖ\Ë ½»RÉ ½» Á ÂÊÁËÌÇÍÎ ½ Ï» for ½>»ZÐ Á ÂÄÑ\Ë Ò for ÐÔ½»NÐ ÁÆÂÓÑ\Ë Á ÂÊÇ Ò (3.5) (3.6) The thirdorder bounds on the Young s modulus have been calculated after determining º» and ¼ƒ» for the three volume fractions of glass. Figure 3.6(a) shows the experimentally determined Young s moduli, the finite element estimates, and thirdorder bounds at a strain rate of 0.001/s for a glassestane composite containing 21% glass beads by volume. At low strain rate and ambient temperatures, there is a considerable difference between the upper and lower bounds. However, at low temperatures close to the glass transition temperature of estane, the stiffening of estane leads to smaller modulus contrast between glass and estane and the bounds are considerably closer. The finite element (FEM) estimates almost coincide with the lower bounds for this volume fraction of glass. Most of the experimental Young s moduli lie below the lower bounds. Figure 3.6(b) shows the results for a strain rate of approximately 2400/s. The high strain rate experimental data for the composites are at a strain rate of approximately 3500/s which is higher than the strain rate used to experimentally determine properties of Estane 5703 (approximately 2400/s strain rate). It is assumed that composite properties do not vary considerably at high strain rates and that the experimental data for the glassestane composites at a strain rate of approximately 3500/s can be compared with
56 41 Young s Modulus (MPa) Strain Rate = 0.001/s Experiment Upper Bound Lower Bound FEM % Glass Temperature ( o C) Young s Modulus (MPa) Strain Rate = 2400/s Experiment 10 1 Upper Bound Lower Bound FEM % Glass Temperature ( o C) (a) Strain Rate = 0.001/s (b) Strain Rate = 2400/s Figure 3.6. Comparison of experimental Young s modulus, bounds and FEM calculations for glassestane composites containing 21% by volume of monodisperse glass beads. predicted values from finite element analyses for a strain rate of approximately 2400/s. From the high strain rate data shown in Figure 3.6(b) it can be observed that the bounds are quite close to each other. This is because of the relatively low modulus contrast between glass and estane at these strain rates. The experimental data are again observed to be considerably lower than the lower bounds except at a temperature of 40 C in which case the experimental value of Young s modulus is two times the finite element estimate and higher than the upper bound. Figure 3.7(a) shows the experimental data, bounds, and finite element estimates of Young s moduli for a glassestane composite containing 44% by volume of glass at a strain rate of 0.001/s. In this case, the finite element estimates are 1.5 to 2 times higher than the lower bounds. However, the experimental data are almost an order of magnitude lower than the finite element estimates. Figure 3.7(b) shows the experimental and predicted Young s moduli at a strain rate of 2400/s. The bounds are quite close to each other and the finite element estimates are slightly higher than the lower bounds, but the experimental data are considerably lower than the lower bounds. The finite element
57 Strain Rate = 0.001/s 10 5 Strain Rate = 2400/s Young s Modulus (MPa) Experiment Upper Bound Lower Bound FEM % Glass Temperature ( o C) Young s Modulus (MPa) Experiment 10 1 Upper Bound Lower Bound FEM % Glass Temperature ( o C) (a) Strain Rate = 0.001/s (b) Strain Rate = 2400/s Figure 3.7. Comparison of experimental Young s modulus, bounds and FEM calculations for glassestane composites containing 44% by volume of monodisperse glass beads. estimates always lie within the thirdorder bounds. Results for the glassestane composite containing 59% by volume of glass are shown in Figures 3.8(a) and 3.8(b). The finite element estimates are higher than the lower bound. The difference between the estimate and the lower bound is larger than for composites with lower volume fractions of glass. At a strain rate of 0.001/s, the experimental data are quite close to the lower bound near room temperature. However, near the glass transition temperature of estane, the experimental Young s modulus is an order of magnitude lower than the finite element estimate and the lower bound. At high strain rates and low temperatures, the difference between finite element predictions and experimental data is less pronounced. However, at high temperatures and high strain rates there is almost an order of magnitude difference between predictions and experiment. The fact that the experimental data are lower than the bounds may indicate that there is considerable debonding of glassbeads from the estane binder. The comparisons between the finite element predictions and experimental data also suggest the assumption of perfect bonding between the glass and the binder is inaccurate. Micrographs of
58 Strain Rate = 0.001/s 10 5 Strain Rate = 2400/s Young s Modulus (MPa) Experiment Upper Bound Lower Bound FEM % Glass Temperature ( o C) Young s Modulus (MPa) Experiment 10 1 Upper Bound Lower Bound FEM % Glass Temperature ( o C) (a) Strain Rate = 0.001/s (b) Strain Rate = 2400/s Figure 3.8. Comparison of experimental Young s modulus, bounds and FEM calculations for glassestane composites containing 59% by volume of monodisperse glass beads. glassestane composites also show that there is some debonding at low strain rates [7]. Damage in the composite appears to play a considerable role in determining ective elastic properties. This damage can be in the form of glassbinder debonds/dewetting, cracking of glass beads or cracking of the binder. Such damage has been observed in glassestane mock PBXs by Cady [7]. The ect of particle debonding on the ective properties is investigated in the next section. The goal is to determine if debonding is adequate to explain the observed discrepancy between finite element estimates and experimentally determined properties of glassestane composites. The high strain rate data on Estane 5703 and the glassestane mock explosives have been determined using stressstrain curves from split Hopkinson pressure bar impact tests. In these tests, the elastic wave moving through a test specimen reaches equilibrium some time after the specimen is impacted. Hence, the initial region of the stressstrain curve may not accurately represent the actual response of the material at small strains. This may be one of the reasons for the high estimates of modulus at high strain rates from finite element simulations. It is also possible that unless the loading history is taken
59 44 into consideration, the ective initial moduli of viscoelastic composites at various strain rates and temperatures cannot be predicted accurately. 3.8 Effect of particle debonding Twodimensional finite element simulations were performed on the microstructure shown in Figures 3.9(a) and 3.9(b) to investigate the ect of particle debonding on ective properties. This microstructure represents a glassestane composite containing 44% glass by volume. Six of the particles in the microstructure are completely contained in the unit cell while the remaining four intersect the boundary. The first set of simulations involved selecting one of the six completely contained particles and completely dissociating it from the surrounding material to simulate a debonded particle. The remainder of the geometry of the unit cell was meshed using sixnoded triangles and the debonded particle was meshed separately. Next, two nodes on diametrically opposite sides of the debonded particle were coupled to the corresponding nodes in the adjacent mesh. The locations of these nodes were chosen so that the line joining the two nodes was perpendicular to the direction of the applied (a) Compression. (b) Tension. Figure 3.9. Debonded particles under (a) compression and (b) tension for a glassestane composite containing 44% by volume of monodisperse glass beads with three debonded particles. Displacements shown are three times the actual. The applied strain is 1%.
60 45 load. Contact elements were created at the hole in the unit cell and at the boundary of the debonded particle. A nonlinear contact simulation was performed on the unit cell with displacement boundary conditions similar to those shown in Figure 3.2. A uniform inward displacement along a boundary was used to simulate compression while a uniform outward displacement was used to simulate tension. The resulting boundary forces and displacements at equilibrium were used in equations (3.2) to compute the ective Young s modulus and Poisson s ratio of the unit cell. The above procedure was repeated five times, with a different particle being debonded from the surrounding material in each simulation. This process was repeated with two, three, four and five debonded particles. Finally, one additional simulation was performed with all six particles debonded from the surrounding material. The deformed shape of a unit cell with three debonded particles under a compressive load is shown in Figure 3.9(a). Figure 3.9(b) shows the deformed shape of the same unit cell under a tensile load. The amount of separation of particles and binder is greater in tension than under compression. The orientation of the gap between the particles and the binder is not always aligned with the direction of applied load and can be affected considerably by the location of adjacent particles. For each simulation, displacements simulating compression were applied first in the Ø direction and then in the Ù direction. The ective Young s moduli in the two directions were averaged to eliminate directional ects. The change in ective compressive Young s modulus with increasing particle debonding can be observed in Figure 3.10(a). The corresponding change in the tensile Young s modulus is shown in Figure 3.10(b). The data points shown in the figure represent the arithmetic mean of the ective moduli predicted for the different combinations of debonded particles at each level of debonding. The standard deviation for each data point is around 10% of the mean. The ective Young s modulus decreases with increasing particlebinder debond. However, under compression, even when 6 of the 10 particles (60% of the particles) have debonded, the ective properties predicted by finite element simulations are still higher than the experimentally determined properties. At the small strains that have been applied (around 1%), it is unlikely that such a high percentage of particles debond in the actual material.
61 46 Young s Modulus (MPa) Strain Rate = 0.001/s Young s Modulus (MPa) 10 5 Strain Rate = 2400/s Temperature ( o C) Temperature ( o C) (a) Compression Strain Rate = 0.001/s Strain Rate = 2400/s Young s Modulus (MPa) Temperature ( o C) Young s Modulus (MPa) (b) Tension Temperature ( o C) Figure Effect of particle debonding on predicted values of Young s modulus of 44% glass/56% estane composite (a) under compression (b) under tension. Ú = Expt. (compression); = FEM  fully bonded; Û = FEM  one particle debonded; Ü = FEM  two particles debonded; Ý = FEM  three particles debonded; = FEM  four particles debonded; Þ = FEM  five particles debonded; Þ!Þ!Þ!Þ!Þ!Þ = FEM  all six particles debonded.
62 47 The high strain rate results show the same qualitative ects as the low strain rate results. The tensile modulus decreases more rapidly with increasing debond than the compressive modulus. The compressive and tensile moduli can be considerably different for glassestane mock PBXs in the presence of debonded particles. Experimental data from tension tests are necessary to validate the tensionbased simulations. 3.9 Summary and conclusions Experimental data on the Young s moduli of extruded Estane 5703 and glassestane mock polymer bonded explosives show strong dependence on temperature and strain rate. Twodimensional finite element simulations based on a unit cell have been performed to determine if the initial modulus of the components of a viscoelastic, glassestane mock polymer bonded explosive can be used to predict the ective initial modulus of the composite. A number of different unit cell sizes were simulated in order to determine appropriate unit cells for the glassestane composites containing three different volume fractions of glass. It has been found that, in two dimensions, unit cells containing five to ten equal sized particles are adequate for the prediction of elastic moduli. A number of threedimensional particle distributions have also been simulated using finite elements. The threedimensional models predict moduli that are around 5% to 10% higher than the twodimensional models. It can be concluded that twodimensional plane strain models estimate elastic moduli of glassestane mock explosives as accurately as threedimensional models. Rigorous thirdorder bounds on the ective elastic properties of the glassestane composites show that the experimental data are close to the lower bounds at low strain rates. This finding suggests that thirdorder lower bounds provide excellent approximations to the ective Young s modulus of low volume fraction composites with high modulus contrast at low strain rates. However, at high strain rates, except at temperatures close to the glass transition temperature of estane, the experimental moduli are considerably lower than the predicted Young s moduli. This finding suggests that there may be substantial debonding and particle/binder fracture in the composites when high strain rate loads are applied.
63 48 Twodimensional finite element simulations of various glassestane composite particle distributions also show that the predicted elastic moduli are considerably higher than the experimentally determined values. This result suggests that there may be particlebinder debonding in the glassestane composites. Simulations performed on a model glassestane particle distribution with increasing particle debonding have shown that increased debonding decreases the ective modulus of the composite. However, even when 60% of the particles have debonded from the surrounding material, the predicted ective moduli are higher than the experimental values. It is unlikely that such a high percentage of the particles would have debonded under the applied strain of around 1%. Therefore, particle debonding cannot fully explain the high moduli obtained from finite element simulations.
64 CHAPTER 4 EFFECTIVE ELASTIC MODULI OF POLYMER BONDED EXPLOSIVES FROM FINITE ELEMENT SIMULATIONS 4.1 Abstract Finite element analysis has been used successfully to estimate the ective properties of many types of composites. The prediction of ective elastic moduli of polymerbonded explosives provides a new challenge. These particulate composites contain extremely high volume fractions of explosive particles (ß 0.9). At room temperature and higher, the Young s modulus of the particles can be 20,000 times that of the binder. Under these conditions, rigorous bounds and analytical approximations for ective elastic properties predict values that are orders of magnitude different from the experimental values. In this work, an approach is presented that can be used to predict threedimensional ective elastic moduli from twodimensional finite element simulations. The approach is validated by comparison with differential ective medium estimates and threedimensional finite element simulations. The twodimensional finite element approach has been used to determine the properties of models of polymer bonded explosives and PBX 9501 in particular, containing high volume fractions of circular and square particles with high modulus contrasts. Results show that estimates of ective elastic properties from twodimensional finite element calculations are close to the values predicted by the differential ective medium approach for a large range of volume fractions and modulus contrasts. Two and threedimensional finite element estimates for volume fractions from 0.7 to 0.9 and found not to differ considerably. Simulations of models of polymer bonded explosives and PBX 9501 show that the microstructure, the amount of discretization, and the type of element used play a considerable role
65 50 in determining the value predicted by finite element simulations. The ective elastic moduli of PBX 9501 predicted by finite element calculations can vary from 200 MPa to 10,000 MPa depending on the microstructure and level of discretization used. The results also suggest that if a microstructure can be found that accurately predicts the elastic properties of PBX 9501 at a certain temperature and strain rate, then the same microstructure can be used to predict elastic properties at other temperatures and strain rates. 4.2 Introduction Experimental determination of the mechanical properties of polymerbonded explosives (PBXs) is hazardous and highly expensive. An alternative to experimentation is the numerical determination of material properties using finite element analysis. PBXs are particulate composites containing explosive particles and a rubbery binder. The particle size distributions in these materials and the mechanical properties of the constituents are required for finite element simulations of the microstructure of these materials. The mechanical properties of the explosive particles can be determined from molecular dynamics simulations. The rubbery binder is amenable to mechanical testing and properties can be determined from laboratory tests. The goal of this work is to investigate if the elastic properties of PBXs can be determined using finite element analyses of PBX microstructures. The major challenges involved in finite element modeling of PBXs are the high volume fraction of particles in PBXs (à1á.â 0.90) and the high modulus contrast between particles and binder (ã]á äãråçæ 10,000 to 20,000) at and above room temperature and at low strain rates. Because of the high volume fractions, microstructures are difficult to generate and even more difficult to digitize from micrographs. Threedimensional finite element models of these materials require considerable computational power. The high modulus contrast leads to large stress concentrations at the interface of particles and the binder. These stress concentrations cannot be simulated adequately without a high degree of mesh discretization. However, detailed numerical simulations are required for the prediction of ective properties of PBXs because rigorous bounds and analytical
66 ï ø ø ø ø ø ú ú ú ú ú ò ø ø ø ø ø ùø ô ø ø ø ø ø ú ú ú ú ú 51 approaches predict values of elastic modulus that are orders of magnitude different from the experimental values. In this work, a procedure is outlined whereby twodimensional finite element simulations can be used to estimate the threedimensional elastic moduli. Finite element estimates on unit cells containing circular particles are compared with differential ective medium estimates of ective elastic moduli for a wide range of volume fractions and modulus contrasts. Twodimensional finite element estimates for selected microstructures are then compared to threedimensional estimates for particle volume fractions of 0.7, 0.75 and 0.8. An appropriate model of PBX 9501 is determined from simulations of manually generated and randomly generated microstructures based on the particle size distribution of PBX Finite element calculations are then performed on this model to estimate the elastic moduli of PBX 9501 for various temperatures and strain rates. 4.3 Finite element approach Numerical determination of the ective properties of particulate composites involves the calculation of the stress and strain fields for a representative volume element (RVE) that simulates the microstructure of the composite. These stresses and strains are averaged over the volume (V) of the RVE and the ective elastic stiffness tensor è of the composite can be calculated from the tensor relation where évê are the stresses and íîqï évêðæñóò è é ê ë9ì évê are the strains. évê ë9ì í î.ô ë9ìõðæñ%ö (4.1) The bulk mechanical response of a random composite is isotropic. However, the size of a RVE than can be simulated numerically is necessarily much smaller than the bulk and may not be isotropic. In this work, it is assumed that the deviation from isotropy of an RVE is small. The stressstrain relation for the RVE can be written in Voigt notation as ï ûüû}ý ïþüþý ïÿüÿý øùƒú ïþüÿý ïÿ}û}ý ï û,þý V V V V V V ûüû û,þ û,ÿ û,þ è þüþ è þüÿ è þüÿ è ÿüÿ è è è è è è è û,ÿ è ôûüû}ý ô}þüþý ô}ÿüÿý øùú ô}þüÿý ô}ÿ}û}ý ôû,þý V V V V V V (4.2)
67 where is the volume average of the quantity. Equation (4.2) can also be inverted and written in terms of the directional Young s moduli, Poisson s ratios and shear moduli as "$#&% V ')( #*% ')( #*% V V ')( #&% "$#&% ')( #*%./ V ')( #&% ')( #*% ",#*% V! "$#*.0 V.0 V + + V "$#*.0 V + V "$#*.0 V %./ V (4.3) where the directional Young s moduli % %, %, and differ by a small amount from the isotropic Young s modulus. Similarly, the mean of the Poisson s ratios (, (, (, (, (, and ( is assumed  to be close to the isotropic Poisson s ratio ( and the mean of the shear moduli , , and is assumed to be close to the isotropic shear  modulus. The determination of ective isotropic elastic modulus of particulate composites using threedimensional finite element analysis therefore requires the determination of volume averaged stresses and strains under appropriate boundary conditions. Once these stresses and strains are known for an RVE, equation (4.3) can be used to determine the ective elastic moduli of the RVE. An investigation into ects of boundary conditions revealed a uniaxial state of stress develops in a RVE when a uniform boundary displacement is applied in one direction and periodicity of boundary displacements is maintained. This means that the ective Young s modulus and Poisson s ratio in a particular direction can be directly computed from equation (4.3) by applying a uniform displacement in that direction. The ective isotropic Young s modulus and Poisson s ratio can then be calculated by averaging the values obtained in the three orthogonal directions from three simulations. The ective shear modulus can be calculated directly from the ective isotropic Young s modulus and Poisson s ratio. The estimation of ective elastic properties from threedimensional simulations is straightforward in principle. However, not only is it difficult to generate RVEs containing high volume fractions of random spherical particles, meshing such threedimensional RVEs is nontrivial. Even if RVEs can be generated and meshed, solution of the finite 52
68 < < ;: 53 element system of equations can be prohibitive in terms of computational expense. A twodimensional approach is described below that requires relatively little computational expense. This approach can be used to arrive at reasonable estimates of threedimensional ective properties of particulate composites. In the twodimensional simulations of particulate composites performed in this study, a crosssection of the composite is chosen that contains the same area fraction of particles as the volume fraction of particles in the composite. Finite element analyses are then performed on this square RVE assuming a state of plane strain. The stressstrain :;=< 1> V D 6 6 EGF H 86 ACB D 6 6 I : K ; 12L3M/ E HF 68 A DB 8 8?$A DB 8 8 I 3M08 87 V I I?$A*J 68 3M/687 V 8 8 F 86 F,, and equation (4.3) can be written in planar or twodimensional form as DB 6 6 B where, D H V H 68 are twodimensional Young s moduli and Poisson s ratios V V (4.4) and different from their threedimensional counterparts. A brief explanation of twodimensional elastic moduli is given in Appendix A. Uniform displacements are applied to the 1 and 2 directions of the RVE and periodic displacements are enforced along the remainder of the boundary to arrive at uniaxial average stresses and the corresponding average strains in the RVE. The ective moduli are calculated using equation (4.4) and D 8ON the directional moduli are averaged to8on arrive at a mean ective Young s modulus ( and a mean ective Poisson s ratio (H ) ) for the RVE. These moduli can also be thought of as ective transverse moduli of a composite containing unidirectional cylinders. It is assumed that these transverse moduli are equal to the twodimensional apparent moduli of an isotropic, homogeneous material subjected to plane strain. Since equation (4.4) is a twodimensional stressstrain law, the twodimensional moduli have to be converted to threedimensional moduli using the relations [31] H D H 2D AQPR?TS H 2D D 2D V? E P H 8WX U U (4.5) (4.6) where H is the ective Poisson s ratio in three dimensions and D is the threedimensional ective Young s modulus.
69 4.4 Validation of approach To determine if the twodimensional finite element simulation approach provides reasonable estimates of threedimensional ective elastic properties of particulate composites, finite element analyses were performed on the twodimensional RVEs containing 10% to 92% by volume of circular particles that are shown in Figure 4.1. The circular particles were placed sequentially at random locations in each RVE such that no two particles were in contact. The particle size distribution in each RVE was based on distributions of the dry blend of PBX 9501 [17]. The Young s modulus of the particles in these finite element simulations was 100,000 MPa and the Poisson s ratio was 0.2. The Young s modulus of the binder was varied from 1 MPa to 10,000 MPa in multiples of 10. The binder Poisson s ratio was chosen to be The ective properties predicted using the finite element analyses were compared with differential ective medium estimates [29, 28]. The differential ective medium approach has been found to provide excellent estimates of elastic properties of particulate composites [28]. Figure 4.2(a) shows ective threedimensional Young s moduli from finite element (FEM) and differential ective medium (DEM) calculations. Figure 4.2(b) shows the corresponding threedimensional Poisson s ratios. The solid lines in the figures are lines of constant modulus contrast between particles and binder and represent the ective elastic property calculated using DEM. The finite element results are shown as squares. The finite element and the DEM predictions are shown to agree remarkably well for all modulus contrasts and for all the simulated volume fractions of particles, implying that the approach described in the previous section gives reasonable estimates of ective elastic properties over a considerable range of volume fractions and modulus contrasts. To obtain a more direct estimate of the ectiveness of the twodimensional models, a second set of finite element simulations was performed on square and cubic RVEs containing particle volume fractions of 0.7, 0.75, and 0.8. The twodimensional RVEs are shown in Figure 4.3(a) and the threedimensional RVEs are shown in Figure 4.3(b). 54
70 55 f p = 0.1 f p = 0.2 f p = 0.3 f p = 0.4 f p = 0.5 f p = 0.6 f p = 0.7 f p = 0.8 f p = 0.92 Figure 4.1. RVEs containing 10% to 92% by volume of circular particles. Y[Z is the volume fraction of particles in a RVE E (MPa) Particle Vol. Frac. (a) Young s Modulus. ν FEM (E b = 1) DEM (E b = 1) 0.35 FEM (E b = 10) DEM (E = 10) b FEM (E = 100) b 0.3 DEM (E = 100) b FEM (E = 1000) b 0.25 DEM (E = 1000) b FEM (E = 10000) b DEM (E = 10000) b Particle Vol. Frac (b)poisson s Ratio. Figure 4.2. Comparison of finite element (FEM) and differential ective medium (DEM) predictions. \^] is the Young s modulus of the binder.
71 56 _`badcqegf _`bahceifkj _`badcqeml (a) Twodimensional RVEs. _`badcqegf _`bahceifkj _`badcqeml (b) Threedimensional RVES. Figure 4.3. Two and threedimensional RVEs containing 70%, 75% and 80% particles by volume. _` is the volume fraction of particles.
72 57 For the twodimensional simulations, each RVE was discretized using sixnoded triangles and approximately 60,000 nodes. Displacement boundary conditions were applied and the average stresses and strain were used to calculate twodimensional ective Young s moduli and Poisson s ratios. The twodimensional moduli were then converted into threedimensional moduli using the approach described in the previous section. The threedimensional RVEs were discretized using 10noded tetrahedral elements with a total of around 100,000 nodes. A uniform displacement was applied perpendicular to one of the faces while the remaining faces were constrained to displace periodically. The threedimensional Young s modulus and Poisson s ratio were directly calculated from the average stresses and strains for these threedimensional models. Figure 4.4(a) shows the ective Young s modulus calculated using the two and threedimensional RVEs shown in Figure 4.3. The Young s modulus used for the particles was 15,300 MPa and the Poisson s ratio was The Young s modulus of the binder was 0.7 MPa and the Poisson s ratio was These values correspond to the moduli of HMX and the binder of PBX 9501 at room temperature and low strain rate [14, 8]. Though the threedimensional models predict higher values of Young s modulus than the twodimensional models, the difference between the two and threedimensional estimates of Young s modulus is small when compared to the modulus contrast between the particles and the binder. Figure 4.4(b) shows the ective Poisson s ratio for the two and threedimensional finite element models. The threedimensional models predict slightly lower values of Poisson s ratio than the twodimensional models. Both two and threedimensional models predict a sharp decrease in Poisson s ratio with increasing particle volume fraction. Comparisons of the twodimensional finite element approach with differential ective medium approximations and threedimensional finite element models suggest that twodimensional analyses provide reasonable approximations of ective properties of particulate composites. Hence, twodimensional models have been used to estimate the ective properties of PBX 9501 in the remainder of this work.
73 58 Young s Modulus (MPa) Two dimensional FEM Three dimensional FEM Particle Vol. Frac. (a) Young s Modulus. Poisson s Ratio Two dimensional FEM Three dimensional FEM Particle Vol. Frac. (b) Poisson s Ratio. Figure 4.4. Two and threedimensional estimates of ective Young s modulus and Poisson s ratio. 4.5 Modeling polymer bonded explosives Most micromechanical calculations for PBXs have been carried out using subgrid models that use highly simplified models of the microstructure (for example, spherical grains coated with binder or spherical voids in an ective PBX material [88]). Closed form solutions from these simple models have been used to provide properties for macroscopic simulations. More detailed calculations have used microstructures containing ordered arrays of circles or polygons in two or three dimensions to model PBXs [52, 89]. These models do not reflect the microstructure of PBXs and hence have limited use for predicting thermoelastic properties. Better twodimensional approximations of the microstructure have been constructed from digital images of the material and used by Benson and Conley [90] to study some aspects of the micromechanics of PBXs. However, such microstructures are extremely difficult to generate and require stateoftheart image processing techniques and excellent images to accurately capture details of the geometry of PBXs. More recently Baer [91] has used a combination of Monte Carlo and molecular dynamics techniques to generate threedimensional microstructures containing spheres and oriented cubes that appear to represent PBX microstructures well. However, the generation of a single realization of these microstructures is very time
74 59 consuming and often leads to a maximum packing fraction of about 70%. Periodicity is also extremely difficult to maintain in the RVEs generated by this method. Both manually and automatically generated twodimensional RVEs of PBX 9501 are discussed in this section. The ective elastic moduli of these RVEs from finite element calculations are then compared with experimentally determined moduli of PBX As in the previous section, the particles in the RVEs represent HMX and have a Young s modulus of 15,300 MPa and a Poisson s ratio of 0.32 [14] and the binder has a Young s modulus of 0.7 MPa and a Poisson s ratio of 0.49 [8]. The ective properties computed from these component properties are compared with the Young s modulus of 1,013 MPa and Poisson s ratio of 0.35 [8] of PBX Manually generated microstructures Figure 4.5 shows six twodimensional microstructures representing PBX Each RVE is filled with particles of various sizes since PBXs are typically a mixture of coarse and fine grains with the finer grains forming a filler between coarser grains. The volume fractions of particles in each of these models is 90n 0.5%. All the models possess square symmetry. The RVEs have also been designed so that particleparticle contact is avoided. Finite element simulations were performed on these RVEs using sixnoded triangular elements such that the geometry of the circular particles was represented accurately. The approach discussed in Section 4.3 was used to determine the ective Young s modulus and Poisson s ratios of these RVEs. Table 4.1 shows the ective Young s modulus and Poisson s ratios of the six RVEs. The values of the ective Young s modulus range from 42 MPa to 192 MPa, with a mean of 132 MPa and a standard deviation of 54 MPa. In comparison, the Young s modulus of PBX 9501 is 1,013 MPa; around 500% to 800% of that predicted using the six RVEs. Among the six RVEs, the Young s modulus appears to be higher for the models with lower amounts of binder along the edges of the RVE. Models 1 through 3 have a single large particle and many smaller particles and show approximately the same ective behavior. Model 4, with a smaller ratio between the radius of the largest and the smallest particles, has a lower ective Young s modulus than the mean value.
75 60 Model 1 Model 2 Model 3 Model 4 Model 5 Model 6 Figure 4.5. Manually generated microstructures containing o 90% circular particles by volume. p is the Young s modulus and q is the Table 4.1. Effective moduli of the six model PBX 9501 microstructures from FEM calculations sixnoded triangular elements. Poisson s ratio. Expt. Model RVE Mean Std. Dev E (MPa) q
76 61 The ective Poisson s ratios of the six RVEs range from 0.25 to 0.34, with a mean of The mean Poisson s ratio of the RVEs is not much different from the measured value for PBX For models 1, 2, and 3, the ective Poisson s ratio is within 10% of that of PBX However, the Poisson s ratio of model 4 is 25% higher and those of models 5 and 6 are 20% and 28% lower than the Poisson s ratio of PBX 9501, respectively. The twodimensional Poisson s ratios of models 4, 5, and 6 are 0.79, 0.39, and 0.33, respectively. In comparison, the twodimensional Poisson s ratio of PBX 9501 is Since, these twodimensional values reflect the actual strains obtained from the twodimensional finite element calculations, it is clear that model 4 is too compliant while models 5 and 6 are too stiff, compared to PBX These observations are in agreement with those made regarding Young s modulus in the previous paragraph and are attributable to the amount of binder along the edge of a RVE. On average, the FEM estimate of Young s modulus is around 13% of the experimentally determined value for PBX The reason for this difference could be that preferential stress paths (stressbridging) in real microstructures lead to increased stiffness. Results shown in Figure 4.4 indicate that the difference between estimates from two and threedimensional models is not large. Hence, it is unlikely that the lower stiffness of the six model RVEs is due to the use of twodimensional models. It is possible that the Young s modulus is underestimated by the six RVEs because the volume fraction of particles in each of these microstructures is lower than 92%. Figure 4.6(a) shows a model containing 92% particles by volume that is a modified version of model 6 in Figure 4.5. The ective Young s modulus of the RVE containing 92% particles is 218 MPa and the ective Poisson s ratio is In comparison, model 6 contains around 90% particles by volume and has an estimated Young s modulus of 192 MPa and a Poisson s ratio of Though there is some increase in the Young s modulus due to increase in particle volume fraction, the value is still around 20% that of PBX Hence, the volume fraction cannot be the only factor leading to underestimation of the Young s modulus by the manually generated microstructures. If a 256r 256 square grid is overlaid on top of the model shown in Figure 4.6(a) and cells in the grid are assigned HMX properties if they contain more than 50% particle
77 62 and binder properties otherwise (referred to as the square grid overlay method ), the new microstructure shown in Figure 4.6(d) is obtained. The RVE in Figure 4.6(d) was modeled using 256 s 256 fournoded square finite elements. The modified model predicts a Young s modulus of 800 MPa and a Poisson s ratio of The modulus is now closer to that of PBX 9501 but the Poisson s ratio is much lower. The stiffer response for the model shown in Figure 4.6(d) is partially due to increased stiffness of fournoded finite elements. To eliminate the possibility that the stiffer response of the modified model is due to element locking caused by the nearly incompressible binder, the binder was also modeled as a twoparameter MooneyRivlin rubber (a) 92% particles. (b) Model 690% particles. (c) Sixnoded Triangles. (d) Fournoded Squares. Figure 4.6. Microstructure containing 92% particles modeled with sixnoded triangles and fournoded squares.
Back to Elements  Tetrahedra vs. Hexahedra
Back to Elements  Tetrahedra vs. Hexahedra Erke Wang, Thomas Nelson, Rainer Rauch CADFEM GmbH, Munich, Germany Abstract This paper presents some analytical results and some test results for different
More informationThe Basics of FEA Procedure
CHAPTER 2 The Basics of FEA Procedure 2.1 Introduction This chapter discusses the spring element, especially for the purpose of introducing various concepts involved in use of the FEA technique. A spring
More informationCOMPUTATIONAL ENGINEERING OF FINITE ELEMENT MODELLING FOR AUTOMOTIVE APPLICATION USING ABAQUS
International Journal of Advanced Research in Engineering and Technology (IJARET) Volume 7, Issue 2, MarchApril 2016, pp. 30 52, Article ID: IJARET_07_02_004 Available online at http://www.iaeme.com/ijaret/issues.asp?jtype=ijaret&vtype=7&itype=2
More informationPlate waves in phononic crystals slabs
Acoustics 8 Paris Plate waves in phononic crystals slabs J.J. Chen and B. Bonello CNRS and Paris VI University, INSP  14 rue de Lourmel, 7515 Paris, France chen99nju@gmail.com 41 Acoustics 8 Paris We
More informationES240 Solid Mechanics Fall 2007. Stress field and momentum balance. Imagine the threedimensional body again. At time t, the material particle ( x, y,
S40 Solid Mechanics Fall 007 Stress field and momentum balance. Imagine the threedimensional bod again. At time t, the material particle,, ) is under a state of stress ij,,, force per unit volume b b,,,.
More informationResearch on the fracture behavior of PBX under static tension
Available online at www.sciencedirect.com ScienceDirect Defence Technology 10 (2014) 154e160 www.elsevier.com/locate/dt Research on the fracture behavior of PBX under static tension Hu GUO*, Jingrun LUO,
More informationFinite Element Formulation for Plates  Handout 3 
Finite Element Formulation for Plates  Handout 3  Dr Fehmi Cirak (fc286@) Completed Version Definitions A plate is a three dimensional solid body with one of the plate dimensions much smaller than the
More informationIntroduction to Solid Modeling Using SolidWorks 2012 SolidWorks Simulation Tutorial Page 1
Introduction to Solid Modeling Using SolidWorks 2012 SolidWorks Simulation Tutorial Page 1 In this tutorial, we will use the SolidWorks Simulation finite element analysis (FEA) program to analyze the response
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationPOISSON AND LAPLACE EQUATIONS. Charles R. O Neill. School of Mechanical and Aerospace Engineering. Oklahoma State University. Stillwater, OK 74078
21 ELLIPTICAL PARTIAL DIFFERENTIAL EQUATIONS: POISSON AND LAPLACE EQUATIONS Charles R. O Neill School of Mechanical and Aerospace Engineering Oklahoma State University Stillwater, OK 74078 2nd Computer
More informationFinite Element Method (ENGC 6321) Syllabus. Second Semester 20132014
Finite Element Method Finite Element Method (ENGC 6321) Syllabus Second Semester 20132014 Objectives Understand the basic theory of the FEM Know the behaviour and usage of each type of elements covered
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationGRADATION OF AGGREGATE FOR CONCRETE BLOCK
GRADATION OF AGGREGATE FOR CONCRETE BLOCK Although numerous papers have been written concerning the proper gradation for concrete mixes, they have generally dealt with plastic mixes, and very little published
More informationThree dimensional thermoset composite curing simulations involving heat conduction, cure kinetics, and viscoelastic stress strain response
Three dimensional thermoset composite curing simulations involving heat conduction, cure kinetics, and viscoelastic stress strain response Harrison Poon, Seid Koric, M. Fouad Ahmad National Center for
More informationAn Overview of the Finite Element Analysis
CHAPTER 1 An Overview of the Finite Element Analysis 1.1 Introduction Finite element analysis (FEA) involves solution of engineering problems using computers. Engineering structures that have complex geometry
More informationPOWDER PROPERTIES LABORATORY
Ground Rules POWDER PROPERTIES LABORATORY You will work as a team of no more than 6 students. At the end of this laboratory session each team will turn in a single report. The report will be reviewed,
More informationChapter Outline. How do atoms arrange themselves to form solids?
Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Simple cubic Facecentered cubic Bodycentered cubic Hexagonal closepacked
More information4.3 Results... 27 4.3.1 Drained Conditions... 27 4.3.2 Undrained Conditions... 28 4.4 References... 30 4.5 Data Files... 30 5 Undrained Analysis of
Table of Contents 1 One Dimensional Compression of a Finite Layer... 3 1.1 Problem Description... 3 1.1.1 Uniform Mesh... 3 1.1.2 Graded Mesh... 5 1.2 Analytical Solution... 6 1.3 Results... 6 1.3.1 Uniform
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationINJECTION MOLDING COOLING TIME REDUCTION AND THERMAL STRESS ANALYSIS
INJECTION MOLDING COOLING TIME REDUCTION AND THERMAL STRESS ANALYSIS Tom Kimerling University of Massachusetts, Amherst MIE 605 Finite Element Analysis Spring 2002 ABSTRACT A FEA transient thermal structural
More informationMETHODS FOR ACHIEVEMENT UNIFORM STRESSES DISTRIBUTION UNDER THE FOUNDATION
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 2, MarchApril 2016, pp. 4566, Article ID: IJCIET_07_02_004 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=2
More informationDifferential Relations for Fluid Flow. Acceleration field of a fluid. The differential equation of mass conservation
Differential Relations for Fluid Flow In this approach, we apply our four basic conservation laws to an infinitesimally small control volume. The differential approach provides point by point details of
More informationFeature Commercial codes Inhouse codes
A simple finite element solver for thermomechanical problems Keywords: Scilab, Open source software, thermoelasticity Introduction In this paper we would like to show how it is possible to develop a
More informationTIE31: Mechanical and thermal properties of optical glass
PAGE 1/10 1 Density The density of optical glass varies from 239 for NBK10 to 603 for SF66 In most cases glasses with higher densities also have higher refractive indices (eg SF type glasses) The density
More informationIntegration of a fin experiment into the undergraduate heat transfer laboratory
Integration of a fin experiment into the undergraduate heat transfer laboratory H. I. AbuMulaweh Mechanical Engineering Department, Purdue University at Fort Wayne, Fort Wayne, IN 46805, USA Email: mulaweh@engr.ipfw.edu
More informationThermoplastic composites
Thermoplastic composites Definition By definition, a thermoplastic is a material based on polymer (macromolecular compound) which can be shaped, in a liquid (viscous) state at a temperature either higher
More informationFinite Elements for 2 D Problems
Finite Elements for 2 D Problems General Formula for the Stiffness Matrix Displacements (u, v) in a plane element are interpolated from nodal displacements (ui, vi) using shape functions Ni as follows,
More informationwww.integratedsoft.com Electromagnetic Sensor Design: Key Considerations when selecting CAE Software
www.integratedsoft.com Electromagnetic Sensor Design: Key Considerations when selecting CAE Software Content Executive Summary... 3 Characteristics of Electromagnetic Sensor Systems... 3 Basic Selection
More informationComposite Design Fundamentals. David Richardson
Composite Design Fundamentals David Richardson Contents A review of the fundamental characteristics of composites Stiffness and Strength Anisotropic Role of fibre, matrix and interface Composite failure
More informationSolved with COMSOL Multiphysics 4.3
Vibrating String Introduction In the following example you compute the natural frequencies of a pretensioned string using the 2D Truss interface. This is an example of stress stiffening ; in fact the
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationIntroduction to Engineering System Dynamics
CHAPTER 0 Introduction to Engineering System Dynamics 0.1 INTRODUCTION The objective of an engineering analysis of a dynamic system is prediction of its behaviour or performance. Real dynamic systems are
More informationBuckling of Spherical Shells
31 Buckling of Spherical Shells 31.1 INTRODUCTION By spherical shell, we mean complete spherical configurations, hemispherical heads (such as pressure vessel heads), and shallow spherical caps. In analyses,
More informationElasticity Theory Basics
G22.3033002: Topics in Computer Graphics: Lecture #7 Geometric Modeling New York University Elasticity Theory Basics Lecture #7: 20 October 2003 Lecturer: Denis Zorin Scribe: Adrian Secord, Yotam Gingold
More informationNew approaches in Eurocode 3 efficient global structural design
New approaches in Eurocode 3 efficient global structural design Part 1: 3D model based analysis using general beamcolumn FEM Ferenc Papp* and József Szalai ** * Associate Professor, Department of Structural
More information1. Fluids Mechanics and Fluid Properties. 1.1 Objectives of this section. 1.2 Fluids
1. Fluids Mechanics and Fluid Properties What is fluid mechanics? As its name suggests it is the branch of applied mechanics concerned with the statics and dynamics of fluids  both liquids and gases.
More informationTechnology of EHIS (stamping) applied to the automotive parts production
Laboratory of Applied Mathematics and Mechanics Technology of EHIS (stamping) applied to the automotive parts production Churilova Maria, SaintPetersburg State Polytechnical University Department of Applied
More informationPlates and Shells: Theory and Computation  4D9  Dr Fehmi Cirak (fc286@) Office: Inglis building mezzanine level (INO 31)
Plates and Shells: Theory and Computation  4D9  Dr Fehmi Cirak (fc286@) Office: Inglis building mezzanine level (INO 31) Outline 1! This part of the module consists of seven lectures and will focus
More information820446  ACMSM  Computer Applications in Solids Mechanics
Coordinating unit: 820  EUETIB  Barcelona College of Industrial Engineering Teaching unit: 737  RMEE  Department of Strength of Materials and Structural Engineering Academic year: Degree: 2015 BACHELOR'S
More informationPhysics 9e/Cutnell. correlated to the. College Board AP Physics 1 Course Objectives
Physics 9e/Cutnell correlated to the College Board AP Physics 1 Course Objectives Big Idea 1: Objects and systems have properties such as mass and charge. Systems may have internal structure. Enduring
More informationhttp://libwww.lanl.gov/lapubs/00818430.pdf
LAUR13461 Approved for public release; distribution is unlimited. Title: INFLUENCE OF POLYMER MOLECULAR WEIGHT, TEMPERATURE, AND STRAIN RATE ON THE MECHANICAL PROPERTIES OF PBX 951 Author(s): D.J. Idar,
More informationOverview of Topics. StressStrain Behavior in Concrete. Elastic Behavior. NonLinear Inelastic Behavior. Stress Distribution.
StressStrain Behavior in Concrete Overview of Topics EARLY AGE CONCRETE Plastic shrinkage shrinkage strain associated with early moisture loss Thermal shrinkage shrinkage strain associated with cooling
More informationDer Einfluss thermophysikalischer Daten auf die numerische Simulation von Gießprozessen
Der Einfluss thermophysikalischer Daten auf die numerische Simulation von Gießprozessen Tagung des Arbeitskreises Thermophysik, 4. 5.3.2010 Karlsruhe, Deutschland E. Kaschnitz Österreichisches GießereiInstitut
More informationMesh Moving Techniques for FluidStructure Interactions With Large Displacements
K. Stein Department of Physics, Bethel College, St. Paul, MN 55112 T. Tezduyar Mechanical Engineering, Rice University, MS 321, Houston, TX 77005 R. Benney Natick Soldier Center, Natick, MA 01760 Mesh
More informationCurrent Standard: Mathematical Concepts and Applications Shape, Space, and Measurement Primary
Shape, Space, and Measurement Primary A student shall apply concepts of shape, space, and measurement to solve problems involving two and threedimensional shapes by demonstrating an understanding of:
More informationM n = (DP)m = (25,000)(104.14 g/mol) = 2.60! 10 6 g/mol
14.4 (a) Compute the repeat unit molecular weight of polystyrene. (b) Compute the numberaverage molecular weight for a polystyrene for which the degree of polymerization is 25,000. (a) The repeat unit
More informationHW 10. = 3.3 GPa (483,000 psi)
HW 10 Problem 15.1 Elastic modulus and tensile strength of poly(methyl methacrylate) at room temperature [20 C (68 F)]. Compare these with the corresponding values in Table 15.1. Figure 15.3 is accurate;
More informationPredictive Modeling of Composite Materials & Structures: StateoftheArt Solutions and Future Challenges.
Predictive Modeling of Composite Materials & Structures: StateoftheArt Solutions and Future Challenges. Roger A. Assaker Roger.Assaker@eXstream.com www.exstream.com Short Abstract Computer Aided Engineering
More informationBUCKLING OF BARS, PLATES, AND SHELLS. Virginia Polytechnic Institute and State University Biacksburg, Virginia 240610219
BUCKLING OF BARS, PLATES, AND SHELLS ROBERT M. JONES Science and Mechanics Professor Emeritus of Engineering Virginia Polytechnic Institute and State University Biacksburg, Virginia 240610219 Bull Ridge
More informationKINETIC MOLECULAR THEORY OF MATTER
KINETIC MOLECULAR THEORY OF MATTER The kineticmolecular theory is based on the idea that particles of matter are always in motion. The theory can be used to explain the properties of solids, liquids,
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationThe elements used in commercial codes can be classified in two basic categories:
CHAPTER 3 Truss Element 3.1 Introduction The single most important concept in understanding FEA, is the basic understanding of various finite elements that we employ in an analysis. Elements are used for
More informationVersion default Titre : SSNP161 Essais biaxiaux de Kupfer Date : 10/10/2012 Page : 1/8 Responsable : François HAMON Clé : V6.03.161 Révision : 9783
Titre : SSNP161 Essais biaxiaux de Kupfer Date : 10/10/2012 Page : 1/8 SSNP161 Biaxial tests of Summarized Kupfer: Kupfer [1] was interested to characterize the performances of the concrete under biaxial
More informationIn mathematics, there are four attainment targets: using and applying mathematics; number and algebra; shape, space and measures, and handling data.
MATHEMATICS: THE LEVEL DESCRIPTIONS In mathematics, there are four attainment targets: using and applying mathematics; number and algebra; shape, space and measures, and handling data. Attainment target
More informationExpress Introductory Training in ANSYS Fluent Lecture 1 Introduction to the CFD Methodology
Express Introductory Training in ANSYS Fluent Lecture 1 Introduction to the CFD Methodology Dimitrios Sofialidis Technical Manager, SimTec Ltd. Mechanical Engineer, PhD PRACE Autumn School 2013  Industry
More informationPaper Pulp Dewatering
Paper Pulp Dewatering Dr. Stefan Rief stefan.rief@itwm.fraunhofer.de Flow and Transport in Industrial Porous Media November 1216, 2007 Utrecht University Overview Introduction and Motivation Derivation
More informationProgramming the Finite Element Method
Programming the Finite Element Method FOURTH EDITION I. M. Smith University of Manchester, UK D. V. Griffiths Colorado School of Mines, USA John Wiley & Sons, Ltd Contents Preface Acknowledgement xv xvii
More informationANALYSIS OF A LAP JOINT FRICTION CONNECTION USING HIGH STRENGTH BOLTS
Nordic Steel Construction Conference 212 Hotel Bristol, Oslo, Norway 57 September 212 ANALYSIS OF A LAP JOINT FRICTION CONNECTION USING HIGH STRENGTH BOLTS Marouene Limam a, Christine Heistermann a and
More informationPragmatic multiscale and multiphysics analysis of Charles Bridge in Prague
Pragmatic multiscale and multiphysics analysis of Charles Bridge in Prague Jiří Šejnoha 1,2 Michal Šejnoha 1,2 Jan Zeman 1 Jan Novák 1,2 with Zdeněk Janda, Jiří Maděra, Jan Vorel and Jan Sýkora 1 Department
More informationEFFECTS ON NUMBER OF CABLES FOR MODAL ANALYSIS OF CABLESTAYED BRIDGES
EFFECTS ON NUMBER OF CABLES FOR MODAL ANALYSIS OF CABLESTAYED BRIDGES YangCheng Wang Associate Professor & Chairman Department of Civil Engineering Chinese Military Academy FengShan 83000,Taiwan Republic
More informationState of Stress at Point
State of Stress at Point Einstein Notation The basic idea of Einstein notation is that a covector and a vector can form a scalar: This is typically written as an explicit sum: According to this convention,
More informationAPPLIED MATHEMATICS ADVANCED LEVEL
APPLIED MATHEMATICS ADVANCED LEVEL INTRODUCTION This syllabus serves to examine candidates knowledge and skills in introductory mathematical and statistical methods, and their applications. For applications
More informationInstitute of Actuaries of India Subject CT3 Probability and Mathematical Statistics
Institute of Actuaries of India Subject CT3 Probability and Mathematical Statistics For 2015 Examinations Aim The aim of the Probability and Mathematical Statistics subject is to provide a grounding in
More informationME6130 An introduction to CFD 11
ME6130 An introduction to CFD 11 What is CFD? Computational fluid dynamics (CFD) is the science of predicting fluid flow, heat and mass transfer, chemical reactions, and related phenomena by solving numerically
More informationFinite Element Formulation for Beams  Handout 2 
Finite Element Formulation for Beams  Handout 2  Dr Fehmi Cirak (fc286@) Completed Version Review of EulerBernoulli Beam Physical beam model midline Beam domain in threedimensions Midline, also called
More informationTWODIMENSIONAL FINITE ELEMENT ANALYSIS OF FORCED CONVECTION FLOW AND HEAT TRANSFER IN A LAMINAR CHANNEL FLOW
TWODIMENSIONAL FINITE ELEMENT ANALYSIS OF FORCED CONVECTION FLOW AND HEAT TRANSFER IN A LAMINAR CHANNEL FLOW Rajesh Khatri 1, 1 M.Tech Scholar, Department of Mechanical Engineering, S.A.T.I., vidisha
More informationSTUDY OF DAMRESERVOIR DYNAMIC INTERACTION USING VIBRATION TESTS ON A PHYSICAL MODEL
STUDY OF DAMRESERVOIR DYNAMIC INTERACTION USING VIBRATION TESTS ON A PHYSICAL MODEL Paulo Mendes, Instituto Superior de Engenharia de Lisboa, Portugal Sérgio Oliveira, Laboratório Nacional de Engenharia
More informationMicroscopy and Nanoindentation. Combining Orientation Imaging. to investigate localized. deformation behaviour. Felix Reinauer
Combining Orientation Imaging Microscopy and Nanoindentation to investigate localized deformation behaviour Felix Reinauer René de Kloe Matt Nowell Introduction Anisotropy in crystalline materials Presentation
More informationAMPLITUDE AND FORCE PROFILING: STUDIES IN ULTRASONIC WELDING OF THERMOPLASTICS
AMPLITUDE AND FORCE PROFILING: STUDIES IN ULTRASONIC WELDING OF THERMOPLASTICS David A. Grewell Branson Ultrasonics Corporation ABSTRACT This paper reviews effects of amplitude and force control during
More informationCylinder Head Gasket Contact Pressure Simulation for a Hermetic Compressor
Purdue University Purdue epubs International Compressor Engineering Conference School of Mechanical Engineering 2006 Cylinder Head Gasket Contact Pressure Simulation for a Hermetic Compressor Pavan P.
More informationCh. 4: Imperfections in Solids Part 1. Dr. Feras Fraige
Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationMesh Discretization Error and Criteria for Accuracy of Finite Element Solutions
Mesh Discretization Error and Criteria for Accuracy of Finite Element Solutions Chandresh Shah Cummins, Inc. Abstract Any finite element analysis performed by an engineer is subject to several types of
More informationCFD Application on Food Industry; Energy Saving on the Bread Oven
MiddleEast Journal of Scientific Research 13 (8): 10951100, 2013 ISSN 19909233 IDOSI Publications, 2013 DOI: 10.5829/idosi.mejsr.2013.13.8.548 CFD Application on Food Industry; Energy Saving on the
More informationMechanical Properties  Stresses & Strains
Mechanical Properties  Stresses & Strains Types of Deformation : Elasic Plastic Anelastic Elastic deformation is defined as instantaneous recoverable deformation Hooke's law : For tensile loading, σ =
More informationMeasurement of Residual Stress in Plastics
Measurement of Residual Stress in Plastics An evaluation has been made of the effectiveness of the chemical probe and hole drilling techniques to measure the residual stresses present in thermoplastic
More informationStrip Flatness Prediction in a 4 High Tandem Mill Using a Dynamic Model.
Strip Flatness Prediction in a 4 High Tandem Mill Using a Dynamic Model. M. A. BelloGomez 1, M. P. GuerreroMata 1, L. A. Leduc Lezama 1, T. P. Berber Solano 1, L. Nieves 2, F. Gonzalez 2, H. R. Siller
More informationFundamentals of grain boundaries and grain boundary migration
1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which
More informationINTRODUCTION TO SOIL MODULI. JeanLouis BRIAUD 1
INTRODUCTION TO SOIL MODULI By JeanLouis BRIAUD 1 The modulus of a soil is one of the most difficult soil parameters to estimate because it depends on so many factors. Therefore when one says for example:
More informationStudies on the Effect of Ageing on a range of UK Polymer Bonded Explosives
Studies on the Effect of Ageing on a range of UK Polymer Bonded Explosives Philip Cheese, Peter Barnes, Michael Sharp DOSG Ron Hollands and Ian Murray BAE Systems Nigel Davies and Peter Jemmet RMCS Shrivenham
More informationCHAPTER 4 4 NUMERICAL ANALYSIS
41 CHAPTER 4 4 NUMERICAL ANALYSIS Simulation is a powerful tool that engineers use to predict the result of a phenomenon or to simulate the working situation in which a part or machine will perform in
More informationFigure 1 EMTAP 42 Tube Test  Electrically Heated
Cookoff testing of pressed PBXs Philip Cheese, Nathan White, Tom Reeves (UK MOD, Defence Equipment and Support), Tony Rowlands (Chemring UK) Chris Stennett (Defence Academy of the UK) Introduction The
More informationAdaptation of General Purpose CFD Code for Fusion MHD Applications*
Adaptation of General Purpose CFD Code for Fusion MHD Applications* Andrei Khodak Princeton Plasma Physics Laboratory P.O. Box 451 Princeton, NJ, 08540 USA akhodak@pppl.gov Abstract Analysis of many fusion
More information7.2.4 Seismic velocity, attenuation and rock properties
7.2.4 Seismic velocity, attenuation and rock properties Rock properties that affect seismic velocity Porosity Lithification Pressure Fluid saturation Velocity in unconsolidated near surface soils (the
More informationMultiBlock Gridding Technique for FLOW3D Flow Science, Inc. July 2004
FSI02TN59R2 MultiBlock Gridding Technique for FLOW3D Flow Science, Inc. July 2004 1. Introduction A major new extension of the capabilities of FLOW3D  the multiblock grid model  has been incorporated
More informationA STUDY ON BONDING STRENGTH OF POLYMERIC FIBERS TO CEMENTITIOUS MATRIX
CD01006 A STUDY ON BONDING STRENGTH OF POLYMERIC FIBERS TO CEMENTITIOUS MATRIX H.R. Pakravan 1, M. Jamshidi 2, M. Latifi 3 1 M.Sc. student, Textile Engineering Department, Amirkabir University, Tehran,
More informationCalculation of Sourcedetector Solid Angle, Using Monte Carlo Method, for Radioactive Sources with Various Geometries and Cylindrical Detector
International Journal of Pure and Applied Physics ISSN 09731776 Volume 3, Number 2 (2007), pp. 201 208 Research India Publications http://www.ripublication.com/ijpap.htm Calculation of Sourcedetector
More informationLecture 19: Eutectoid Transformation in Steels: a typical case of Cellular
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationMATH. ALGEBRA I HONORS 9 th Grade 12003200 ALGEBRA I HONORS
* Students who scored a Level 3 or above on the Florida Assessment Test Math Florida Standards (FSAMAFS) are strongly encouraged to make Advanced Placement and/or dual enrollment courses their first choices
More informationMECHANICS OF SOLIDS  BEAMS TUTORIAL 1 STRESSES IN BEAMS DUE TO BENDING. On completion of this tutorial you should be able to do the following.
MECHANICS OF SOLIDS  BEAMS TUTOIAL 1 STESSES IN BEAMS DUE TO BENDING This is the first tutorial on bending of beams designed for anyone wishing to study it at a fairly advanced level. You should judge
More informationThe Role of Electric Polarization in Nonlinear optics
The Role of Electric Polarization in Nonlinear optics Sumith Doluweera Department of Physics University of Cincinnati Cincinnati, Ohio 45221 Abstract Nonlinear optics became a very active field of research
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationAs published in PIM International
As published in PIM International www.piminternational.com 64 Powder Injection Moulding International September 2012 Rapid prototyping of highperformance ceramics opens new opportunities for the CIM industry
More informationMaterial Deformations. Academic Resource Center
Material Deformations Academic Resource Center Agenda Origin of deformations Deformations & dislocations Dislocation motion Slip systems Stresses involved with deformation Deformation by twinning Origin
More information3D WAVEGUIDE MODELING AND SIMULATION USING SBFEM
3D WAVEGUIDE MODELING AND SIMULATION USING SBFEM Fabian Krome, Hauke Gravenkamp BAM Federal Institute for Materials Research and Testing, Unter den Eichen 87, 12205 Berlin, Germany email: Fabian.Krome@BAM.de
More informationHigh Performance Castable CL20 Explosive
High Performance Castable CL20 Explosive Prepared For 2004 IM/EM Technical Symposium November 1517, 2004 San Francisco, CA Robert L Hatch OUTLINE Background and Objectives Theoretical Performance Processing
More informationScalars, Vectors and Tensors
Scalars, Vectors and Tensors A scalar is a physical quantity that it represented by a dimensional number at a particular point in space and time. Examples are hydrostatic pressure and temperature. A vector
More informationMultiphase Flow  Appendices
Discovery Laboratory Multiphase Flow  Appendices 1. Creating a Mesh 1.1. What is a geometry? The geometry used in a CFD simulation defines the problem domain and boundaries; it is the area (2D) or volume
More informationStress Relaxation Study of Paper and Plastic Film based Packaging Material
Master's Degree Thesis ISRN: BTHAMTEX2009/D02SE Stress Relaxation Study of Paper and Plastic Film based Packaging Material Rajdip Roy Lu Qi Department of Mechanical Engineering Blekinge Institute
More information